# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2016

data_njy1
_audit_creation_date              2015-09-26
_audit_creation_method
;
Olex2 1.2
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_publ_contact_author_address      ?
_publ_contact_author_email        ?
_publ_contact_author_name         ''
_publ_contact_author_phone        ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2008). Acta Cryst. A64, 112-122.
;
_chemical_name_common             ?
_chemical_name_systematic         ?
_chemical_formula_moiety          '0.5(K28 Na12 Nb64 Ni20 O324), 21(O)'
_chemical_formula_sum             'H43 K14 Na6 Nb32 Ni10 O183'
_chemical_formula_weight          7216.90
_chemical_melting_point           ?
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H' 'H' 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K' 'K' 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ni' 'Ni' 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Nb' 'Nb' -2.0727 0.6215
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na' 'Na' 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system       'monoclinic'
_space_group_IT_number            12
_space_group_name_H-M_alt         'I 1 2/m 1'
_space_group_name_Hall            '-I 2y'
loop_
  _space_group_symop_operation_xyz
 'x, y, z'
 '-x, y, -z'
 'x+1/2, y+1/2, z+1/2'
 '-x+1/2, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x, -y, z'
 '-x+1/2, -y+1/2, -z+1/2'
 'x+1/2, -y+1/2, z+1/2'

_cell_length_a                    15.1399(14)
_cell_length_b                    24.824(2)
_cell_length_c                    25.190(3)
_cell_angle_alpha                 90
_cell_angle_beta                  103.469(2)
_cell_angle_gamma                 90
_cell_volume                      9206.8(17)
_cell_formula_units_Z             2
_cell_measurement_reflns_used     9299
_cell_measurement_temperature     296(2)
_cell_measurement_theta_max       28.47
_cell_measurement_theta_min       2.18
_shelx_estimated_absorpt_T_max    0.488
_shelx_estimated_absorpt_T_min    0.362
_exptl_absorpt_coefficient_mu     3.355
_exptl_absorpt_correction_T_max   0.7457
_exptl_absorpt_correction_T_min   0.5951
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_process_details
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.0761 before and 0.0527 after correction.
The Ratio of minimum to maximum transmission is 0.7980.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details    ?
_exptl_crystal_colour             green
_exptl_crystal_density_diffrn     2.603
_exptl_crystal_density_meas       .
_exptl_crystal_density_method     ?
_exptl_crystal_description        block
_exptl_crystal_F_000              6862
_exptl_crystal_size_max           0.38
_exptl_crystal_size_mid           0.27
_exptl_crystal_size_min           0.25
_exptl_transmission_factor_max    ?
_exptl_transmission_factor_min    ?
_diffrn_reflns_av_R_equivalents   0.0322
_diffrn_reflns_av_unetI/netI      0.0393
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max        16
_diffrn_reflns_limit_h_min        -18
_diffrn_reflns_limit_k_max        29
_diffrn_reflns_limit_k_min        -29
_diffrn_reflns_limit_l_max        30
_diffrn_reflns_limit_l_min        -19
_diffrn_reflns_number             23133
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full         25.242
_diffrn_reflns_theta_max          25.249
_diffrn_reflns_theta_min          2.069
_diffrn_ambient_temperature       296.15
_diffrn_detector_area_resol_mean  ?
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type   'Bruker APEX-II CCD'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_radiation_monochromator   'graphite'
_diffrn_radiation_type            MoK\a
_diffrn_radiation_wavelength      0.71073
_diffrn_source                    ?
_diffrn_standards_number          0
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_full     .
_reflns_Friedel_fraction_max      .
_reflns_number_gt                 5917
_reflns_number_total              8541
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression      'I > 2σ(I)'
_computing_cell_refinement        'Bruker SAINT'
_computing_data_collection        'Bruker APEX2'
_computing_data_reduction         'Bruker SAINT'
_computing_molecular_graphics     'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material   'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement   'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution     'SHELXL-2008 (Sheldrick, 2008)'
_refine_diff_density_max          2.107
_refine_diff_density_min          -1.587
_refine_diff_density_rms          0.245
_refine_ls_extinction_coef        .
_refine_ls_extinction_method      none
_refine_ls_goodness_of_fit_ref    1.053
_refine_ls_hydrogen_treatment     undef
_refine_ls_matrix_type            full
_refine_ls_number_parameters      567
_refine_ls_number_reflns          8541
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0893
_refine_ls_R_factor_gt            0.0572
_refine_ls_restrained_S_all       1.053
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0564P)²+430.1892P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme       calc
_refine_ls_wR_factor_gt           0.1330
_refine_ls_wR_factor_ref          0.1646
_refine_special_details           ?
_olex2_refinement_description
;
1. Others
 Fixed Sof: K6(0.5) O20W(0.5) O21W(0.25) O22W(0.5)
;
_atom_sites_solution_hydrogens    .
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    ?
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_site_symmetry_order
  _atom_site_calc_flag
  _atom_site_refinement_flags_posn
  _atom_site_refinement_flags_adp
  _atom_site_refinement_flags_occupancy
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 Nb1 Nb 0.98218(6) 0.26810(3) 0.06567(3) 0.0166(2) Uani 1 1 d . . . . .
 Nb2 Nb 1.15861(6) 0.20096(3) 0.03640(4) 0.0216(2) Uani 1 1 d . . . . .
 Nb3 Nb 0.98278(7) 0.13403(3) 0.06342(4) 0.0234(2) Uani 1 1 d . . . . .
 Nb4 Nb 0.83182(6) 0.43320(3) 0.07205(3) 0.0159(2) Uani 1 1 d . . . . .
 Nb5 Nb 0.65827(8) 0.5000 0.10112(5) 0.0233(3) Uani 1 2 d S T P . .
 Nb6 Nb 0.79745(6) 0.43261(3) 0.20132(4) 0.0203(2) Uani 1 1 d . . . . .
 Nb7 Nb 1.10841(6) 0.43285(3) 0.13581(3) 0.01436(19) Uani 1 1 d . . . . .
 Nb8 Nb 1.07143(6) 0.43268(3) 0.26401(3) 0.0181(2) Uani 1 1 d . . . . .
 Nb9 Nb 1.24710(8) 0.5000 0.23583(5) 0.0190(3) Uani 1 2 d S T P . .
 Ni1 Ni 1.14333(8) 0.32802(5) 0.03305(5) 0.0189(3) Uani 1 1 d . . . . .
 Ni2 Ni 0.95248(8) 0.37150(5) 0.16767(5) 0.0181(3) Uani 1 1 d . . . . .
 Ni3 Ni 0.95266(11) 0.5000 0.16730(6) 0.0130(3) Uani 1 2 d S T P . .
 K1 K 1.0000 0.43277(12) 0.0000 0.0262(7) Uani 1 2 d S T P . .
 K2 K 1.4839(2) 0.41220(13) 0.27714(14) 0.0598(9) Uani 1 1 d . . . . .
 K3 K 1.3998(4) 0.5000 0.3799(2) 0.0811(16) Uani 1 2 d S T P . .
 K4 K 0.8372(4) 0.0000 0.1038(3) 0.0854(17) Uani 1 2 d S T P . .
 K5 K 1.2742(4) 0.5000 0.0715(2) 0.094(2) Uani 1 2 d S T P . .
 K6 K 1.0923(4) 0.3815(2) 0.4243(2) 0.0447(13) Uiso 0.5 1 d . . . . .
 Na1 Na 1.1567(3) 0.21322(17) 0.26239(19) 0.0389(11) Uani 1 1 d . . . . .
 Na2 Na 1.2316(6) 0.5000 0.4582(3) 0.058(2) Uani 1 2 d S T P . .
 O1 O 1.0000 0.3151(3) 0.0000 0.0176(19) Uani 1 2 d S T P . .
 O2 O 0.9384(4) 0.4370(2) 0.2195(3) 0.0188(14) Uani 1 1 d . . . . .
 O3 O 0.9666(4) 0.4366(2) 0.1153(2) 0.0142(13) Uani 1 1 d . . . . .
 O4 O 0.9677(4) 0.3166(3) 0.1141(2) 0.0211(14) Uani 1 1 d . . . . .
 O5 O 0.8435(4) 0.3852(3) 0.0224(3) 0.0217(14) Uani 1 1 d . . . . .
 O6 O 1.1243(4) 0.3852(2) 0.0865(3) 0.0193(14) Uani 1 1 d . . . . .
 O7 O 0.8186(4) 0.3891(3) 0.1373(3) 0.0200(14) Uani 1 1 d . . . . .
 O8 O 0.8174(6) 0.5000 0.1362(4) 0.0159(18) Uani 1 2 d S T P . .
 O9 O 1.1168(5) 0.2616(3) 0.0799(3) 0.0240(15) Uani 1 1 d . . . . .
 O10 O 1.0866(4) 0.3888(2) 0.1985(3) 0.0191(14) Uani 1 1 d . . . . .
 O11 O 1.0888(6) 0.5000 0.1983(3) 0.0169(19) Uani 1 2 d S T P . .
 O12 O 0.8558(5) 0.2618(3) 0.0199(3) 0.0244(15) Uani 1 1 d . . . . .
 O13 O 1.1068(6) 0.5000 0.0935(4) 0.0183(19) Uani 1 2 d S T P . .
 O14 O 0.8530(6) 0.5000 0.0348(4) 0.020(2) Uani 1 2 d S T P . .
 O15 O 1.2029(5) 0.4445(3) 0.2807(3) 0.0224(15) Uani 1 1 d . . . . .
 O16 O 0.9712(5) 0.2019(3) 0.1040(3) 0.0250(15) Uani 1 1 d . . . . .
 O17 O 1.0000 0.2027(3) 0.0000 0.023(2) Uani 1 2 d S T P . .
 O18 O 0.7018(4) 0.4446(3) 0.0550(3) 0.0238(15) Uani 1 1 d . . . . .
 O19 O 0.8549(5) 0.1481(3) 0.0229(3) 0.0293(16) Uani 1 1 d . . . . .
 O20 O 1.2323(4) 0.4454(2) 0.1762(3) 0.0212(14) Uani 1 1 d . . . . .
 O21 O 1.0537(7) 0.5000 0.3004(4) 0.022(2) Uani 1 2 d S T P . .
 O22 O 0.7960(6) 0.5000 0.2415(4) 0.025(2) Uani 1 2 d S T P . .
 O23 O 1.1169(5) 0.1484(3) 0.0828(3) 0.0279(16) Uani 1 1 d . . . . .
 O24 O 1.2785(5) 0.2026(3) 0.0641(3) 0.0361(18) Uani 1 1 d . . . . .
 O25 O 0.7811(5) 0.3832(3) 0.2487(3) 0.0360(18) Uani 1 1 d . . . . .
 O26 O 1.0000 0.0913(4) 0.0000 0.031(3) Uani 1 2 d S T P . .
 O27 O 1.0623(5) 0.3825(3) 0.3126(3) 0.0324(17) Uani 1 1 d . . . . .
 O28 O 1.3646(6) 0.5000 0.2654(4) 0.030(2) Uani 1 2 d S T P . .
 O29 O 0.6736(5) 0.4446(3) 0.1597(3) 0.0287(16) Uani 1 1 d . . . . .
 O30 O 1.2828(6) 0.3255(4) 0.0652(4) 0.049(2) Uani 1 1 d . . . . .
 O31 O 0.9350(7) 0.3136(3) 0.2228(4) 0.049(2) Uani 1 1 d . . . . .
 O32 O 0.5392(7) 0.5000 0.0750(5) 0.039(3) Uani 1 2 d S T P . .
 O33 O 0.9719(6) 0.0824(3) 0.1097(3) 0.0378(19) Uani 1 1 d . . . . .
 O1W O 1.1754(6) 0.2855(3) 0.1961(3) 0.041(2) Uani 1 1 d . . . . .
 O2W O 0.8878(9) 0.0000 -0.0063(6) 0.051(3) Uani 1 2 d S T P . .
 O3W O 1.2559(7) 0.4347(4) 0.3951(4) 0.060(3) Uani 1 1 d . . . . .
 O4W O 1.1743(7) 0.1432(4) 0.1982(4) 0.058(3) Uani 1 1 d . . . . .
 O5W O 0.7243(8) 0.0702(4) 0.0212(5) 0.069(3) Uani 1 1 d . . . . .
 O6W O 1.3571(7) 0.3648(4) 0.1792(4) 0.060(3) Uani 1 1 d . . . . .
 O7W O 1.3724(8) 0.2229(4) 0.1708(4) 0.066(3) Uani 1 1 d . . . . .
 O8W O 0.9925(8) 0.2003(4) 0.2143(4) 0.063(3) Uani 1 1 d . . . . .
 O9W O 1.0757(12) 0.5000 0.4125(6) 0.078(5) Uani 1 2 d S T P . .
 O10W O 0.7464(8) 0.2950(4) 0.0874(5) 0.072(4) Uani 1 1 d . . . . .
 O11W O 0.5951(8) 0.5770(5) -0.0438(5) 0.088(4) Uani 1 1 d . . . . .
 O12W O 0.7682(11) 0.1862(6) 0.1048(6) 0.104(5) Uani 1 1 d . . . . .
 O13W O 0.5948(14) 0.5000 0.2555(10) 0.107(7) Uani 1 2 d S T P . .
 O14W O 0.5334(11) 0.3816(7) 0.1670(10) 0.168(9) Uani 1 1 d . . . . .
 O15W O 1.4277(15) 0.5000 0.1560(9) 0.150(11) Uani 1 2 d S T P . .
 O16W O 0.4401(13) 0.6591(8) -0.0528(8) 0.156(8) Uani 1 1 d . . . . .
 O17W O 0.5312(16) 0.2663(10) 0.1432(10) 0.187(9) Uiso 1 1 d . . . . .
 O18W O 0.6782(14) 0.4069(9) 0.3262(9) 0.163(8) Uiso 1 1 d . . . . .
 O19W O 0.6760(15) 0.2932(9) 0.2455(10) 0.178(8) Uiso 1 1 d . . . . .
 O20W O 0.9003(18) 0.3585(11) 0.3492(12) 0.096(8) Uiso 0.5 1 d . . . . .
 O21W O 0.868(3) 0.5000 0.347(2) 0.123(15) Uiso 0.5 2 d S T P . .
 O22W O 0.902(3) 0.4236(19) 0.416(2) 0.183(18) Uiso 0.5 1 d . . . . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 Nb1 Nb3 3.3287(11) . ?
 Nb1 Ni1 3.1314(14) 2_755 ?
 Nb1 Ni1 3.1264(15) . ?
 Nb1 O1 2.093(5) . ?
 Nb1 O4 1.765(6) . ?
 Nb1 O9 1.993(7) . ?
 Nb1 O12 1.996(7) . ?
 Nb1 O16 1.932(7) . ?
 Nb1 O17 2.377(6) . ?
 Nb2 Nb3 3.3399(13) . ?
 Nb2 Nb3 3.3404(12) 2_755 ?
 Nb2 Ni1 3.1623(14) . ?
 Nb2 O9 2.046(7) . ?
 Nb2 O12 2.048(7) 2_755 ?
 Nb2 O17 2.3629(10) . ?
 Nb2 O19 1.963(7) 2_755 ?
 Nb2 O23 1.952(7) . ?
 Nb2 O24 1.787(7) . ?
 Nb3 Nb2 3.3403(12) 2_755 ?
 Nb3 Nb3 3.3551(18) 2_755 ?
 Nb3 K2 4.094(4) 7_755 ?
 Nb3 K3 3.885(3) 7_755 ?
 Nb3 O16 2.001(7) . ?
 Nb3 O17 2.392(6) . ?
 Nb3 O19 1.997(7) . ?
 Nb3 O23 2.007(7) . ?
 Nb3 O26 1.985(5) . ?
 Nb3 O33 1.766(7) . ?
 Nb4 Nb4 3.3168(16) 6_565 ?
 Nb4 Nb5 3.3296(14) . ?
 Nb4 Ni2 3.0717(14) . ?
 Nb4 Ni3 3.1320(16) . ?
 Nb4 K1 3.4541(9) . ?
 Nb4 K5 3.963(5) 5_765 ?
 Nb4 O3 2.080(6) . ?
 Nb4 O5 1.767(6) . ?
 Nb4 O7 2.023(6) . ?
 Nb4 O8 2.362(6) . ?
 Nb4 O14 1.968(5) . ?
 Nb4 O18 1.935(7) . ?
 Nb5 Nb4 3.3296(14) 6_565 ?
 Nb5 Nb6 3.3365(14) 6_565 ?
 Nb5 Nb6 3.3366(14) . ?
 Nb5 O8 2.365(9) . ?
 Nb5 O18 2.008(7) . ?
 Nb5 O18 2.008(7) 6_565 ?
 Nb5 O29 1.992(7) . ?
 Nb5 O29 1.992(7) 6_565 ?
 Nb5 O32 1.768(10) . ?
 Nb6 Nb6 3.3460(17) 6_565 ?
 Nb6 Ni2 3.0750(15) . ?
 Nb6 Ni3 3.1612(16) . ?
 Nb6 O2 2.078(6) . ?
 Nb6 O7 2.029(6) . ?
 Nb6 O8 2.410(6) . ?
 Nb6 O22 1.958(5) . ?
 Nb6 O25 1.768(7) . ?
 Nb6 O29 1.947(7) . ?
 Nb7 Nb7 3.3339(15) 6_565 ?
 Nb7 Nb9 3.3273(13) . ?
 Nb7 Ni2 3.0692(14) . ?
 Nb7 Ni3 3.1368(16) . ?
 Nb7 K1 3.4325(9) . ?
 Nb7 K5 3.687(5) . ?
 Nb7 O3 2.089(6) . ?
 Nb7 O6 1.772(6) . ?
 Nb7 O10 2.011(6) . ?
 Nb7 O11 2.358(6) . ?
 Nb7 O13 1.975(5) . ?
 Nb7 O20 1.939(6) . ?
 Nb8 Nb8 3.3423(16) 6_565 ?
 Nb8 Nb9 3.3539(14) . ?
 Nb8 Ni2 3.0664(14) . ?
 Nb8 Ni3 3.1494(16) . ?
 Nb8 K6 4.173(6) . ?
 Nb8 O2 2.068(6) . ?
 Nb8 O10 2.033(6) . ?
 Nb8 O11 2.409(6) . ?
 Nb8 O15 1.958(7) . ?
 Nb8 O21 1.955(5) . ?
 Nb8 O27 1.775(7) . ?
 Nb9 Nb7 3.3273(13) 6_565 ?
 Nb9 Nb8 3.3540(14) 6_565 ?
 Nb9 K2 4.117(4) 6_565 ?
 Nb9 K3 3.821(6) . ?
 Nb9 O11 2.362(9) . ?
 Nb9 O15 1.993(7) . ?
 Nb9 O15 1.993(7) 6_565 ?
 Nb9 O20 1.996(6) 6_565 ?
 Nb9 O20 1.996(6) . ?
 Nb9 O28 1.761(9) . ?
 Ni1 Nb1 3.1315(14) 2_755 ?
 Ni1 K1 3.365(3) . ?
 Ni1 O1 2.1594(18) . ?
 Ni1 O5 2.032(6) 2_755 ?
 Ni1 O6 2.023(6) . ?
 Ni1 O9 2.119(7) . ?
 Ni1 O12 2.118(7) 2_755 ?
 Ni1 O30 2.079(9) . ?
 Ni2 O2 2.127(6) . ?
 Ni2 O3 2.127(6) . ?
 Ni2 O4 1.968(6) . ?
 Ni2 O7 2.040(6) . ?
 Ni2 O10 2.044(6) . ?
 Ni2 O31 2.057(8) . ?
 Ni3 Nb4 3.1321(15) 6_565 ?
 Ni3 Nb7 3.1369(16) 6_565 ?
 Ni3 Nb8 3.1494(16) 6_565 ?
 Ni3 O2 2.087(6) . ?
 Ni3 O2 2.087(6) 6_565 ?
 Ni3 O3 2.090(6) . ?
 Ni3 O3 2.090(6) 6_565 ?
 Ni3 O8 2.015(9) . ?
 Ni3 O11 2.027(9) . ?
 K1 K1 3.338(6) 5_765 ?
 K1 O1 2.920(9) . ?
 K1 O3 3.064(6) 2_755 ?
 K1 O3 3.064(6) . ?
 K1 O5 2.819(7) 2_755 ?
 K1 O5 2.819(7) . ?
 K1 O6 2.788(6) . ?
 K1 O6 2.788(6) 2_755 ?
 K1 O13 3.030(8) . ?
 K1 O13 3.029(8) 5_765 ?
 K1 O14 3.068(8) . ?
 K1 O14 3.068(8) 5_765 ?
 K2 Nb3 4.094(4) 7_755 ?
 K2 K3 3.822(6) . ?
 K2 Na1 3.772(6) 7_755 ?
 K2 O28 2.802(7) . ?
 K2 O33 2.775(8) 7_755 ?
 K2 O4W 2.952(11) 7_755 ?
 K2 O6W 2.992(11) . ?
 K2 O8W 2.818(11) 7_755 ?
 K2 O13W 2.880(13) 1_655 ?
 K2 O14W 3.13(2) 1_655 ?
 K2 O18W 2.92(2) 1_655 ?
 K3 Nb3 3.885(3) 4_755 ?
 K3 Nb3 3.885(3) 7_755 ?
 K3 K2 3.822(6) 6_565 ?
 K3 Na2 3.566(11) . ?
 K3 O28 2.808(13) . ?
 K3 O33 2.791(9) 4_755 ?
 K3 O33 2.791(9) 7_755 ?
 K3 O2W 2.914(16) 3 ?
 K3 O3W 2.811(13) 6_565 ?
 K3 O3W 2.811(13) . ?
 K4 K2 4.160(6) 4_745 ?
 K4 K2 4.160(6) 7_755 ?
 K4 K3 3.907(9) 7_755 ?
 K4 Na2 3.644(10) 3_444 ?
 K4 O33 2.869(9) . ?
 K4 O33 2.869(9) 6 ?
 K4 O2W 3.044(16) . ?
 K4 O5W 2.936(13) . ?
 K4 O5W 2.936(13) 6 ?
 K4 O18W 2.95(2) 7_655 ?
 K4 O18W 2.95(2) 4_645 ?
 K5 Nb4 3.963(5) 5_765 ?
 K5 Nb4 3.963(5) 2_755 ?
 K5 Nb7 3.687(5) 6_565 ?
 K5 O13 2.717(10) . ?
 K5 O14 2.912(11) 5_765 ?
 K5 O20 3.157(8) . ?
 K5 O20 3.157(8) 6_565 ?
 K5 O11W 2.949(15) 5_765 ?
 K5 O11W 2.949(15) 2_755 ?
 K5 O15W 2.76(2) . ?
 K6 Na2 3.603(8) . ?
 K6 O24 2.829(9) 7_755 ?
 K6 O27 2.743(9) . ?
 K6 O3W 3.044(13) . ?
 K6 O5W 3.020(13) 8 ?
 K6 O9W 2.960(6) . ?
 K6 O20W 3.13(3) . ?
 K6 O22W 3.02(5) . ?
 Na1 K2 3.772(6) 7_755 ?
 Na1 Na1 3.538(9) 7_755 ?
 Na1 O1W 2.513(10) 7_755 ?
 Na1 O1W 2.511(9) . ?
 Na1 O4W 2.431(10) . ?
 Na1 O6W 2.470(11) 7_755 ?
 Na1 O7W 2.426(11) 7_755 ?
 Na1 O8W 2.520(12) . ?
 Na2 K4 3.644(10) 3 ?
 Na2 K6 3.603(8) 6_565 ?
 Na2 O2W 2.326(16) 3 ?
 Na2 O3W 2.359(11) . ?
 Na2 O3W 2.359(11) 6_565 ?
 Na2 O5W 2.376(12) 3 ?
 Na2 O5W 2.376(12) 8 ?
 Na2 O9W 2.372(19) . ?
 O1 Nb1 2.093(5) 2_755 ?
 O1 Ni1 2.1595(18) 2_755 ?
 O5 Ni1 2.032(6) 2_755 ?
 O8 Nb4 2.362(6) 6_565 ?
 O8 Nb6 2.410(6) 6_565 ?
 O11 Nb7 2.358(6) 6_565 ?
 O11 Nb8 2.409(6) 6_565 ?
 O12 Nb2 2.049(7) 2_755 ?
 O12 Ni1 2.118(7) 2_755 ?
 O13 Nb7 1.975(5) 6_565 ?
 O13 K1 3.030(8) 5_765 ?
 O14 Nb4 1.968(5) 6_565 ?
 O14 K1 3.068(8) 5_765 ?
 O14 K5 2.912(11) 5_765 ?
 O17 Nb1 2.377(6) 2_755 ?
 O17 Nb2 2.3629(10) 2_755 ?
 O17 Nb3 2.392(6) 2_755 ?
 O19 Nb2 1.963(7) 2_755 ?
 O21 Nb8 1.955(5) 6_565 ?
 O22 Nb6 1.959(5) 6_565 ?
 O24 K6 2.829(9) 7_755 ?
 O26 Nb3 1.985(5) 2_755 ?
 O28 K2 2.802(7) 6_565 ?
 O33 K2 2.775(8) 7_755 ?
 O33 K3 2.791(9) 7_755 ?
 O1W Na1 2.513(10) 7_755 ?
 O2W K3 2.914(15) 3_444 ?
 O2W Na2 2.326(16) 3_444 ?
 O4W K2 2.952(11) 7_755 ?
 O5W K6 3.020(13) 8_454 ?
 O5W Na2 2.376(12) 3_444 ?
 O6W Na1 2.470(11) 7_755 ?
 O7W Na1 2.426(11) 7_755 ?
 O8W K2 2.818(11) 7_755 ?
 O9W K6 2.960(6) 6_565 ?
 O11W K5 2.949(15) 5_765 ?
 O13W K2 2.880(13) 1_455 ?
 O13W K2 2.880(13) 6_465 ?
 O14W K2 3.13(2) 1_455 ?
 O18W K2 2.92(2) 1_455 ?
 O18W K4 2.95(2) 7_655 ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 Ni1 Nb1 Nb3 117.71(4) 2_755 . ?
 Ni1 Nb1 Nb3 117.77(4) . . ?
 Ni1 Nb1 Ni1 86.08(4) . 2_755 ?
 O1 Nb1 Nb3 122.9(2) . . ?
 O1 Nb1 Ni1 43.51(4) . . ?
 O1 Nb1 Ni1 43.41(4) . 2_755 ?
 O1 Nb1 O17 77.0(3) . . ?
 O4 Nb1 Nb3 134.1(2) . . ?
 O4 Nb1 Ni1 95.0(2) . . ?
 O4 Nb1 Ni1 94.3(2) . 2_755 ?
 O4 Nb1 O1 103.1(3) . . ?
 O4 Nb1 O9 102.6(3) . . ?
 O4 Nb1 O12 101.3(3) . . ?
 O4 Nb1 O16 101.2(3) . . ?
 O4 Nb1 O17 179.4(2) . . ?
 O9 Nb1 Nb3 85.15(19) . . ?
 O9 Nb1 Ni1 42.03(19) . . ?
 O9 Nb1 Ni1 125.96(19) . 2_755 ?
 O9 Nb1 O1 82.66(19) . . ?
 O9 Nb1 O12 154.2(3) . . ?
 O9 Nb1 O17 78.0(2) . . ?
 O12 Nb1 Nb3 85.31(19) . . ?
 O12 Nb1 Ni1 125.92(19) . . ?
 O12 Nb1 Ni1 41.91(19) . 2_755 ?
 O12 Nb1 O1 82.5(2) . . ?
 O12 Nb1 O17 78.1(2) . . ?
 O16 Nb1 Nb3 32.8(2) . . ?
 O16 Nb1 Ni1 134.4(2) . . ?
 O16 Nb1 Ni1 133.9(2) . 2_755 ?
 O16 Nb1 O1 155.7(3) . . ?
 O16 Nb1 O9 92.6(3) . . ?
 O16 Nb1 O12 92.3(3) . . ?
 O16 Nb1 O17 78.7(3) . . ?
 O17 Nb1 Nb3 45.92(15) . . ?
 O17 Nb1 Ni1 85.30(12) . 2_755 ?
 O17 Nb1 Ni1 85.41(12) . . ?
 Nb3 Nb2 Nb3 60.30(3) . 2_755 ?
 Ni1 Nb2 Nb3 116.41(4) . . ?
 Ni1 Nb2 Nb3 116.48(4) . 2_755 ?
 O9 Nb2 Nb3 123.02(19) . 2_755 ?
 O9 Nb2 Nb3 84.07(19) . . ?
 O9 Nb2 Ni1 41.47(19) . . ?
 O9 Nb2 O12 80.3(3) . 2_755 ?
 O9 Nb2 O17 77.4(2) . . ?
 O12 Nb2 Nb3 84.22(19) 2_755 2_755 ?
 O12 Nb2 Nb3 123.1(2) 2_755 . ?
 O12 Nb2 Ni1 41.46(19) 2_755 . ?
 O12 Nb2 O17 77.5(3) 2_755 . ?
 O17 Nb2 Nb3 45.73(15) . . ?
 O17 Nb2 Nb3 45.72(15) . 2_755 ?
 O17 Nb2 Ni1 84.8(2) . . ?
 O19 Nb2 Nb3 82.9(2) 2_755 . ?
 O19 Nb2 Nb3 32.8(2) 2_755 2_755 ?
 O19 Nb2 Ni1 130.7(2) 2_755 . ?
 O19 Nb2 O9 155.3(3) 2_755 . ?
 O19 Nb2 O12 89.5(3) 2_755 2_755 ?
 O19 Nb2 O17 78.5(3) 2_755 . ?
 O23 Nb2 Nb3 83.0(2) . 2_755 ?
 O23 Nb2 Nb3 33.0(2) . . ?
 O23 Nb2 Ni1 130.6(2) . . ?
 O23 Nb2 O9 89.3(3) . . ?
 O23 Nb2 O12 155.5(3) . 2_755 ?
 O23 Nb2 O17 78.7(3) . . ?
 O23 Nb2 O19 91.0(3) . 2_755 ?
 O24 Nb2 Nb3 136.0(3) . 2_755 ?
 O24 Nb2 Nb3 135.8(3) . . ?
 O24 Nb2 Ni1 92.8(3) . . ?
 O24 Nb2 O9 100.8(3) . . ?
 O24 Nb2 O12 100.9(3) . 2_755 ?
 O24 Nb2 O17 177.7(3) . . ?
 O24 Nb2 O19 103.2(3) . 2_755 ?
 O24 Nb2 O23 102.8(3) . . ?
 Nb1 Nb3 Nb2 60.77(2) . 2_755 ?
 Nb1 Nb3 Nb2 60.76(3) . . ?
 Nb1 Nb3 Nb3 91.02(2) . 2_755 ?
 Nb1 Nb3 K2 105.30(5) . 7_755 ?
 Nb1 Nb3 K3 148.54(9) . 7_755 ?
 Nb2 Nb3 Nb2 90.04(3) . 2_755 ?
 Nb2 Nb3 Nb3 59.84(3) 2_755 2_755 ?
 Nb2 Nb3 Nb3 59.86(3) . 2_755 ?
 Nb2 Nb3 K2 142.08(6) 2_755 7_755 ?
 Nb2 Nb3 K2 114.67(6) . 7_755 ?
 Nb2 Nb3 K3 149.43(8) 2_755 7_755 ?
 Nb2 Nb3 K3 100.52(9) . 7_755 ?
 Nb3 Nb3 K2 157.42(6) 2_755 7_755 ?
 Nb3 Nb3 K3 101.00(9) 2_755 7_755 ?
 K3 Nb3 K2 57.17(9) 7_755 7_755 ?
 O16 Nb3 Nb1 31.56(19) . . ?
 O16 Nb3 Nb2 81.29(19) . 2_755 ?
 O16 Nb3 Nb2 81.6(2) . . ?
 O16 Nb3 Nb3 122.58(19) . 2_755 ?
 O16 Nb3 K2 74.94(19) . 7_755 ?
 O16 Nb3 K3 128.4(2) . 7_755 ?
 O16 Nb3 O17 77.1(2) . . ?
 O16 Nb3 O23 86.0(3) . . ?
 O17 Nb3 Nb1 45.56(15) . . ?
 O17 Nb3 Nb2 45.02(2) . 2_755 ?
 O17 Nb3 Nb2 45.03(2) . . ?
 O17 Nb3 Nb3 45.46(15) . 2_755 ?
 O17 Nb3 K2 147.93(14) . 7_755 ?
 O17 Nb3 K3 138.10(14) . 7_755 ?
 O19 Nb3 Nb1 80.06(19) . . ?
 O19 Nb3 Nb2 32.2(2) . 2_755 ?
 O19 Nb3 Nb2 122.2(2) . . ?
 O19 Nb3 Nb3 82.0(2) . 2_755 ?
 O19 Nb3 K2 115.7(2) . 7_755 ?
 O19 Nb3 K3 130.1(2) . 7_755 ?
 O19 Nb3 O16 85.6(3) . . ?
 O19 Nb3 O17 77.1(2) . . ?
 O19 Nb3 O23 154.0(3) . . ?
 O23 Nb3 Nb1 79.91(19) . . ?
 O23 Nb3 Nb2 121.97(19) . 2_755 ?
 O23 Nb3 Nb2 31.98(19) . . ?
 O23 Nb3 Nb3 81.9(2) . 2_755 ?
 O23 Nb3 K2 85.7(2) . 7_755 ?
 O23 Nb3 K3 73.3(2) . 7_755 ?
 O23 Nb3 O17 76.95(19) . . ?
 O26 Nb3 Nb1 123.4(2) . . ?
 O26 Nb3 Nb2 80.88(15) . 2_755 ?
 O26 Nb3 Nb2 80.90(15) . . ?
 O26 Nb3 Nb3 32.3(2) . 2_755 ?
 O26 Nb3 K2 129.1(2) . 7_755 ?
 O26 Nb3 K3 72.7(2) . 7_755 ?
 O26 Nb3 O16 154.9(3) . . ?
 O26 Nb3 O17 77.8(3) . . ?
 O26 Nb3 O19 88.6(2) . . ?
 O26 Nb3 O23 88.6(2) . . ?
 O33 Nb3 Nb1 135.5(3) . . ?
 O33 Nb3 Nb2 135.7(3) . 2_755 ?
 O33 Nb3 Nb2 134.2(3) . . ?
 O33 Nb3 Nb3 133.5(3) . 2_755 ?
 O33 Nb3 K2 32.6(3) . 7_755 ?
 O33 Nb3 K3 40.6(3) . 7_755 ?
 O33 Nb3 O16 103.9(3) . . ?
 O33 Nb3 O17 178.7(3) . . ?
 O33 Nb3 O19 103.7(3) . . ?
 O33 Nb3 O23 102.3(3) . . ?
 O33 Nb3 O26 101.1(3) . . ?
 Nb4 Nb4 Nb5 60.126(17) 6_565 . ?
 Nb4 Nb4 K1 90.18(5) 6_565 . ?
 Nb4 Nb4 K5 65.26(4) 6_565 5_765 ?
 Nb5 Nb4 K1 146.42(5) . . ?
 Nb5 Nb4 K5 79.60(7) . 5_765 ?
 Ni2 Nb4 Nb4 119.91(3) . 6_565 ?
 Ni2 Nb4 Nb5 115.57(4) . . ?
 Ni2 Nb4 Ni3 61.88(3) . . ?
 Ni2 Nb4 K1 91.94(4) . . ?
 Ni2 Nb4 K5 164.77(8) . 5_765 ?
 Ni3 Nb4 Nb4 58.03(2) . 6_565 ?
 Ni3 Nb4 Nb5 85.29(4) . . ?
 Ni3 Nb4 K1 91.92(5) . . ?
 Ni3 Nb4 K5 121.18(5) . 5_765 ?
 K1 Nb4 K5 73.34(8) . 5_765 ?
 O3 Nb4 Nb4 87.70(16) . 6_565 ?
 O3 Nb4 Nb5 126.39(17) . . ?
 O3 Nb4 Ni2 43.71(17) . . ?
 O3 Nb4 Ni3 41.44(16) . . ?
 O3 Nb4 K1 61.43(17) . . ?
 O3 Nb4 K5 126.95(18) . 5_765 ?
 O3 Nb4 O8 81.3(3) . . ?
 O5 Nb4 Nb4 132.4(2) . 6_565 ?
 O5 Nb4 Nb5 134.9(2) . . ?
 O5 Nb4 Ni2 94.6(2) . . ?
 O5 Nb4 Ni3 139.7(2) . . ?
 O5 Nb4 K1 54.4(2) . . ?
 O5 Nb4 K5 73.9(2) . 5_765 ?
 O5 Nb4 O3 98.6(3) . . ?
 O5 Nb4 O7 104.8(3) . . ?
 O5 Nb4 O8 177.8(3) . . ?
 O5 Nb4 O14 100.2(3) . . ?
 O5 Nb4 O18 101.9(3) . . ?
 O7 Nb4 Nb4 122.79(18) . 6_565 ?
 O7 Nb4 Nb5 81.88(18) . . ?
 O7 Nb4 Ni2 41.10(18) . . ?
 O7 Nb4 Ni3 79.36(18) . . ?
 O7 Nb4 K1 130.51(18) . . ?
 O7 Nb4 K5 150.7(2) . 5_765 ?
 O7 Nb4 O3 82.3(2) . . ?
 O7 Nb4 O8 77.4(2) . . ?
 O8 Nb4 Nb4 45.39(15) . 6_565 ?
 O8 Nb4 Nb5 45.3(2) . . ?
 O8 Nb4 Ni2 86.92(18) . . ?
 O8 Nb4 Ni3 40.0(2) . . ?
 O8 Nb4 K1 123.99(19) . . ?
 O8 Nb4 K5 104.39(17) . 5_765 ?
 O14 Nb4 Nb4 32.6(2) . 6_565 ?
 O14 Nb4 Nb5 84.8(2) . . ?
 O14 Nb4 Ni2 131.3(3) . . ?
 O14 Nb4 Ni3 77.8(3) . . ?
 O14 Nb4 K1 62.0(2) . . ?
 O14 Nb4 K5 44.7(3) . 5_765 ?
 O14 Nb4 O3 88.1(3) . . ?
 O14 Nb4 O7 154.3(3) . . ?
 O14 Nb4 O8 77.7(3) . . ?
 O18 Nb4 Nb4 81.6(2) . 6_565 ?
 O18 Nb4 Nb5 33.1(2) . . ?
 O18 Nb4 Ni2 129.4(2) . . ?
 O18 Nb4 Ni3 118.4(2) . . ?
 O18 Nb4 K1 136.1(2) . . ?
 O18 Nb4 K5 64.0(2) . 5_765 ?
 O18 Nb4 O3 159.0(3) . . ?
 O18 Nb4 O7 88.3(3) . . ?
 O18 Nb4 O8 78.3(3) . . ?
 O18 Nb4 O14 92.4(3) . . ?
 Nb4 Nb5 Nb4 59.75(3) 6_565 . ?
 Nb4 Nb5 Nb6 91.40(4) 6_565 . ?
 Nb4 Nb5 Nb6 61.64(3) 6_565 6_565 ?
 Nb4 Nb5 Nb6 61.64(3) . . ?
 Nb4 Nb5 Nb6 91.40(4) . 6_565 ?
 Nb6 Nb5 Nb6 60.19(4) 6_565 . ?
 O8 Nb5 Nb4 45.17(15) . 6_565 ?
 O8 Nb5 Nb4 45.17(15) . . ?
 O8 Nb5 Nb6 46.23(15) . 6_565 ?
 O8 Nb5 Nb6 46.23(15) . . ?
 O18 Nb5 Nb4 31.73(19) 6_565 6_565 ?
 O18 Nb5 Nb4 31.73(19) . . ?
 O18 Nb5 Nb4 80.34(19) 6_565 . ?
 O18 Nb5 Nb4 80.34(19) . 6_565 ?
 O18 Nb5 Nb6 123.12(19) 6_565 . ?
 O18 Nb5 Nb6 123.12(19) . 6_565 ?
 O18 Nb5 Nb6 81.90(19) 6_565 6_565 ?
 O18 Nb5 Nb6 81.90(19) . . ?
 O18 Nb5 O8 76.9(2) 6_565 . ?
 O18 Nb5 O8 76.9(2) . . ?
 O18 Nb5 O18 86.5(4) . 6_565 ?
 O29 Nb5 Nb4 81.8(2) . . ?
 O29 Nb5 Nb4 123.1(2) . 6_565 ?
 O29 Nb5 Nb4 81.8(2) 6_565 6_565 ?
 O29 Nb5 Nb4 123.1(2) 6_565 . ?
 O29 Nb5 Nb6 31.7(2) 6_565 6_565 ?
 O29 Nb5 Nb6 80.9(2) 6_565 . ?
 O29 Nb5 Nb6 31.7(2) . . ?
 O29 Nb5 Nb6 80.9(2) . 6_565 ?
 O29 Nb5 O8 77.9(3) . . ?
 O29 Nb5 O8 77.9(3) 6_565 . ?
 O29 Nb5 O18 87.6(3) 6_565 6_565 ?
 O29 Nb5 O18 154.8(3) . 6_565 ?
 O29 Nb5 O18 87.6(3) . . ?
 O29 Nb5 O18 154.8(3) 6_565 . ?
 O29 Nb5 O29 87.4(4) 6_565 . ?
 O32 Nb5 Nb4 134.9(3) . . ?
 O32 Nb5 Nb4 134.9(3) . 6_565 ?
 O32 Nb5 Nb6 133.7(3) . . ?
 O32 Nb5 Nb6 133.7(3) . 6_565 ?
 O32 Nb5 O8 179.8(4) . . ?
 O32 Nb5 O18 103.2(3) . . ?
 O32 Nb5 O18 103.2(3) . 6_565 ?
 O32 Nb5 O29 102.0(3) . 6_565 ?
 O32 Nb5 O29 102.0(3) . . ?
 Nb5 Nb6 Nb6 59.905(18) . 6_565 ?
 Ni2 Nb6 Nb5 115.27(4) . . ?
 Ni2 Nb6 Nb6 119.56(3) . 6_565 ?
 Ni2 Nb6 Ni3 61.51(3) . . ?
 Ni3 Nb6 Nb5 84.72(4) . . ?
 Ni3 Nb6 Nb6 58.05(2) . 6_565 ?
 O2 Nb6 Nb5 125.13(17) . . ?
 O2 Nb6 Nb6 86.99(17) . 6_565 ?
 O2 Nb6 Ni2 43.64(18) . . ?
 O2 Nb6 Ni3 40.72(17) . . ?
 O2 Nb6 O8 80.1(3) . . ?
 O7 Nb6 Nb5 81.63(18) . . ?
 O7 Nb6 Nb6 122.21(18) . 6_565 ?
 O7 Nb6 Ni2 41.05(18) . . ?
 O7 Nb6 Ni3 78.55(18) . . ?
 O7 Nb6 O2 81.9(3) . . ?
 O7 Nb6 O8 76.2(2) . . ?
 O8 Nb6 Nb5 45.1(2) . . ?
 O8 Nb6 Nb6 46.04(14) . 6_565 ?
 O8 Nb6 Ni2 86.01(17) . . ?
 O8 Nb6 Ni3 39.6(2) . . ?
 O22 Nb6 Nb5 83.2(3) . . ?
 O22 Nb6 Nb6 31.3(2) . 6_565 ?
 O22 Nb6 Ni2 131.7(3) . . ?
 O22 Nb6 Ni3 77.7(3) . . ?
 O22 Nb6 O2 88.6(3) . . ?
 O22 Nb6 O7 152.8(3) . . ?
 O22 Nb6 O8 77.1(3) . . ?
 O25 Nb6 Nb5 134.0(3) . . ?
 O25 Nb6 Nb6 133.9(3) . 6_565 ?
 O25 Nb6 Ni2 94.6(3) . . ?
 O25 Nb6 Ni3 141.2(3) . . ?
 O25 Nb6 O2 100.7(3) . . ?
 O25 Nb6 O7 103.9(3) . . ?
 O25 Nb6 O8 179.2(3) . . ?
 O25 Nb6 O22 102.9(4) . . ?
 O25 Nb6 O29 101.5(3) . . ?
 O29 Nb6 Nb5 32.5(2) . . ?
 O29 Nb6 Nb6 81.2(2) . 6_565 ?
 O29 Nb6 Ni2 128.9(2) . . ?
 O29 Nb6 Ni3 117.2(2) . . ?
 O29 Nb6 O2 157.2(3) . . ?
 O29 Nb6 O7 87.9(3) . . ?
 O29 Nb6 O8 77.6(3) . . ?
 O29 Nb6 O22 91.3(3) . . ?
 Nb7 Nb7 K1 90.03(5) 6_565 . ?
 Nb7 Nb7 K5 63.12(4) 6_565 . ?
 Nb9 Nb7 Nb7 59.934(17) . 6_565 ?
 Nb9 Nb7 K1 145.68(5) . . ?
 Nb9 Nb7 K5 74.46(9) . . ?
 Ni2 Nb7 Nb7 119.75(3) . 6_565 ?
 Ni2 Nb7 Nb9 116.03(4) . . ?
 Ni2 Nb7 Ni3 61.85(3) . . ?
 Ni2 Nb7 K1 92.41(4) . . ?
 Ni2 Nb7 K5 169.42(9) . . ?
 Ni3 Nb7 Nb7 57.90(2) . 6_565 ?
 Ni3 Nb7 Nb9 85.48(4) . . ?
 Ni3 Nb7 K1 92.25(4) . . ?
 Ni3 Nb7 K5 119.97(5) . . ?
 K1 Nb7 K5 77.23(9) . . ?
 O3 Nb7 Nb7 87.48(16) . 6_565 ?
 O3 Nb7 Nb9 126.57(17) . . ?
 O3 Nb7 Ni2 43.78(17) . . ?
 O3 Nb7 Ni3 41.37(16) . . ?
 O3 Nb7 K1 61.88(17) . . ?
 O3 Nb7 K5 129.56(19) . . ?
 O3 Nb7 O11 81.5(3) . . ?
 O6 Nb7 Nb7 131.9(2) . 6_565 ?
 O6 Nb7 Nb9 134.5(2) . . ?
 O6 Nb7 Ni2 95.2(2) . . ?
 O6 Nb7 Ni3 139.9(2) . . ?
 O6 Nb7 K1 54.0(2) . . ?
 O6 Nb7 K5 77.1(2) . . ?
 O6 Nb7 O3 99.0(3) . . ?
 O6 Nb7 O10 105.2(3) . . ?
 O6 Nb7 O11 176.9(3) . . ?
 O6 Nb7 O13 99.9(3) . . ?
 O6 Nb7 O20 101.7(3) . . ?
 O10 Nb7 Nb7 122.93(18) . 6_565 ?
 O10 Nb7 Nb9 82.38(18) . . ?
 O10 Nb7 Ni2 41.21(18) . . ?
 O10 Nb7 Ni3 79.60(18) . . ?
 O10 Nb7 K1 130.92(19) . . ?
 O10 Nb7 K5 147.6(2) . . ?
 O10 Nb7 O3 82.6(2) . . ?
 O10 Nb7 O11 77.9(2) . . ?
 O11 Nb7 Nb7 45.02(15) . 6_565 ?
 O11 Nb7 Nb9 45.2(2) . . ?
 O11 Nb7 Ni2 87.27(19) . . ?
 O11 Nb7 Ni3 40.3(2) . . ?
 O11 Nb7 K1 124.09(18) . . ?
 O11 Nb7 K5 100.24(19) . . ?
 O13 Nb7 Nb7 32.4(2) . 6_565 ?
 O13 Nb7 Nb9 84.9(2) . . ?
 O13 Nb7 Ni2 130.3(3) . . ?
 O13 Nb7 Ni3 76.9(2) . . ?
 O13 Nb7 K1 61.3(2) . . ?
 O13 Nb7 K5 46.0(3) . . ?
 O13 Nb7 O3 87.0(3) . . ?
 O13 Nb7 O10 154.0(3) . . ?
 O13 Nb7 O11 77.0(3) . . ?
 O20 Nb7 Nb7 80.73(18) . 6_565 ?
 O20 Nb7 Nb9 32.81(19) . . ?
 O20 Nb7 Ni2 130.7(2) . . ?
 O20 Nb7 Ni3 118.3(2) . . ?
 O20 Nb7 K1 134.6(2) . . ?
 O20 Nb7 K5 58.9(2) . . ?
 O20 Nb7 O3 159.2(3) . . ?
 O20 Nb7 O10 89.5(3) . . ?
 O20 Nb7 O11 78.0(3) . . ?
 O20 Nb7 O13 92.0(3) . . ?
 Nb8 Nb8 Nb9 60.116(18) 6_565 . ?
 Nb8 Nb8 K6 107.71(8) 6_565 . ?
 Nb9 Nb8 K6 118.10(8) . . ?
 Ni2 Nb8 Nb8 119.69(3) . 6_565 ?
 Ni2 Nb8 Nb9 115.33(4) . . ?
 Ni2 Nb8 Ni3 61.74(3) . . ?
 Ni2 Nb8 K6 120.87(9) . . ?
 Ni3 Nb8 Nb8 57.95(2) . 6_565 ?
 Ni3 Nb8 Nb9 84.84(4) . . ?
 Ni3 Nb8 K6 144.16(9) . . ?
 O2 Nb8 Nb8 87.03(17) . 6_565 ?
 O2 Nb8 Nb9 125.45(17) . . ?
 O2 Nb8 Ni2 43.79(18) . . ?
 O2 Nb8 Ni3 40.93(17) . . ?
 O2 Nb8 K6 112.64(19) . . ?
 O2 Nb8 O11 80.8(3) . . ?
 O10 Nb8 Nb8 122.37(17) . 6_565 ?
 O10 Nb8 Nb9 81.38(18) . . ?
 O10 Nb8 Ni2 41.36(18) . . ?
 O10 Nb8 Ni3 78.98(17) . . ?
 O10 Nb8 K6 128.63(19) . . ?
 O10 Nb8 O2 82.4(3) . . ?
 O10 Nb8 O11 76.3(2) . . ?
 O11 Nb8 Nb8 46.08(15) . 6_565 ?
 O11 Nb8 Nb9 44.8(2) . . ?
 O11 Nb8 Ni2 86.45(17) . . ?
 O11 Nb8 Ni3 40.1(2) . . ?
 O11 Nb8 K6 151.62(17) . . ?
 O15 Nb8 Nb8 81.35(18) . 6_565 ?
 O15 Nb8 Nb9 32.22(18) . . ?
 O15 Nb8 Ni2 128.6(2) . . ?
 O15 Nb8 Ni3 117.04(19) . . ?
 O15 Nb8 K6 89.7(2) . . ?
 O15 Nb8 O2 157.2(3) . . ?
 O15 Nb8 O10 87.3(3) . . ?
 O15 Nb8 O11 77.0(3) . . ?
 O21 Nb8 Nb8 31.3(2) . 6_565 ?
 O21 Nb8 Nb9 82.9(3) . . ?
 O21 Nb8 Ni2 132.5(3) . . ?
 O21 Nb8 Ni3 78.1(3) . . ?
 O21 Nb8 K6 78.1(2) . . ?
 O21 Nb8 O2 89.3(3) . . ?
 O21 Nb8 O10 153.2(3) . . ?
 O21 Nb8 O11 77.2(3) . . ?
 O21 Nb8 O15 90.8(3) . . ?
 O27 Nb8 Nb8 134.6(2) . 6_565 ?
 O27 Nb8 Nb9 133.5(3) . . ?
 O27 Nb8 Ni2 94.1(2) . . ?
 O27 Nb8 Ni3 141.6(3) . . ?
 O27 Nb8 K6 28.3(2) . . ?
 O27 Nb8 O2 100.8(3) . . ?
 O27 Nb8 O10 103.0(3) . . ?
 O27 Nb8 O11 178.2(3) . . ?
 O27 Nb8 O15 101.3(3) . . ?
 O27 Nb8 O21 103.6(3) . . ?
 Nb7 Nb9 Nb7 60.13(3) . 6_565 ?
 Nb7 Nb9 Nb8 61.25(3) 6_565 6_565 ?
 Nb7 Nb9 Nb8 91.04(4) . 6_565 ?
 Nb7 Nb9 Nb8 91.04(4) 6_565 . ?
 Nb7 Nb9 Nb8 61.25(3) . . ?
 Nb7 Nb9 K2 106.55(5) 6_565 6_565 ?
 Nb7 Nb9 K2 144.63(6) . 6_565 ?
 Nb7 Nb9 K3 148.70(3) 6_565 . ?
 Nb7 Nb9 K3 148.70(3) . . ?
 Nb8 Nb9 Nb8 59.77(4) . 6_565 ?
 Nb8 Nb9 K2 111.68(5) 6_565 6_565 ?
 Nb8 Nb9 K2 153.78(6) . 6_565 ?
 Nb8 Nb9 K3 97.65(9) . . ?
 Nb8 Nb9 K3 97.65(9) 6_565 . ?
 K3 Nb9 K2 57.42(9) . 6_565 ?
 O11 Nb9 Nb7 45.13(15) . 6_565 ?
 O11 Nb9 Nb7 45.13(15) . . ?
 O11 Nb9 Nb8 45.91(16) . 6_565 ?
 O11 Nb9 Nb8 45.91(16) . . ?
 O11 Nb9 K2 147.52(6) . 6_565 ?
 O11 Nb9 K3 135.5(2) . . ?
 O15 Nb9 Nb7 81.19(18) . . ?
 O15 Nb9 Nb7 81.19(18) 6_565 6_565 ?
 O15 Nb9 Nb7 122.62(19) 6_565 . ?
 O15 Nb9 Nb7 122.63(19) . 6_565 ?
 O15 Nb9 Nb8 31.59(19) . . ?
 O15 Nb9 Nb8 31.59(19) 6_565 6_565 ?
 O15 Nb9 Nb8 80.6(2) 6_565 . ?
 O15 Nb9 Nb8 80.6(2) . 6_565 ?
 O15 Nb9 K2 83.0(2) 6_565 6_565 ?
 O15 Nb9 K2 127.61(19) . 6_565 ?
 O15 Nb9 K3 70.8(2) 6_565 . ?
 O15 Nb9 K3 70.8(2) . . ?
 O15 Nb9 O11 77.5(2) 6_565 . ?
 O15 Nb9 O11 77.5(2) . . ?
 O15 Nb9 O15 87.4(4) . 6_565 ?
 O15 Nb9 O20 87.9(3) 6_565 6_565 ?
 O15 Nb9 O20 154.4(3) . 6_565 ?
 O15 Nb9 O20 87.9(3) . . ?
 O15 Nb9 O20 154.4(3) 6_565 . ?
 O20 Nb9 Nb7 31.76(19) 6_565 6_565 ?
 O20 Nb9 Nb7 31.76(19) . . ?
 O20 Nb9 Nb7 80.19(18) . 6_565 ?
 O20 Nb9 Nb7 80.19(19) 6_565 . ?
 O20 Nb9 Nb8 122.80(19) 6_565 . ?
 O20 Nb9 Nb8 82.27(19) 6_565 6_565 ?
 O20 Nb9 Nb8 122.80(19) . 6_565 ?
 O20 Nb9 Nb8 82.27(19) . . ?
 O20 Nb9 K2 76.67(19) 6_565 6_565 ?
 O20 Nb9 K2 119.2(2) . 6_565 ?
 O20 Nb9 K3 130.67(19) . . ?
 O20 Nb9 K3 130.67(19) 6_565 . ?
 O20 Nb9 O11 76.9(2) 6_565 . ?
 O20 Nb9 O11 76.9(2) . . ?
 O20 Nb9 O20 85.5(4) 6_565 . ?
 O28 Nb9 Nb7 135.8(3) . . ?
 O28 Nb9 Nb7 135.8(3) . 6_565 ?
 O28 Nb9 Nb8 133.1(3) . 6_565 ?
 O28 Nb9 Nb8 133.1(3) . . ?
 O28 Nb9 K2 32.74(9) . 6_565 ?
 O28 Nb9 K3 43.1(4) . . ?
 O28 Nb9 O11 178.6(4) . . ?
 O28 Nb9 O15 101.5(3) . 6_565 ?
 O28 Nb9 O15 101.5(3) . . ?
 O28 Nb9 O20 104.1(3) . . ?
 O28 Nb9 O20 104.1(3) . 6_565 ?
 Nb1 Ni1 Nb1 67.44(4) . 2_755 ?
 Nb1 Ni1 Nb2 64.86(3) . . ?
 Nb1 Ni1 Nb2 64.82(3) 2_755 . ?
 Nb1 Ni1 K1 86.19(4) 2_755 . ?
 Nb1 Ni1 K1 86.27(4) . . ?
 Nb2 Ni1 K1 144.72(6) . . ?
 O1 Ni1 Nb1 41.75(13) . 2_755 ?
 O1 Ni1 Nb1 41.85(13) . . ?
 O1 Ni1 Nb2 85.6(2) . . ?
 O1 Ni1 K1 59.1(2) . . ?
 O5 Ni1 Nb1 136.05(19) 2_755 . ?
 O5 Ni1 Nb1 85.67(19) 2_755 2_755 ?
 O5 Ni1 Nb2 134.13(19) 2_755 . ?
 O5 Ni1 K1 56.73(19) 2_755 . ?
 O5 Ni1 O1 95.1(2) 2_755 . ?
 O5 Ni1 O9 170.7(3) 2_755 . ?
 O5 Ni1 O12 95.3(3) 2_755 2_755 ?
 O5 Ni1 O30 92.1(3) 2_755 . ?
 O6 Ni1 Nb1 135.07(19) . 2_755 ?
 O6 Ni1 Nb1 85.32(18) . . ?
 O6 Ni1 Nb2 134.68(19) . . ?
 O6 Ni1 K1 55.86(18) . . ?
 O6 Ni1 O1 94.3(2) . . ?
 O6 Ni1 O5 91.1(3) . 2_755 ?
 O6 Ni1 O9 95.8(3) . . ?
 O6 Ni1 O12 170.5(3) . 2_755 ?
 O6 Ni1 O30 92.9(3) . . ?
 O9 Ni1 Nb1 85.05(18) . 2_755 ?
 O9 Ni1 Nb1 39.02(18) . . ?
 O9 Ni1 Nb2 39.76(19) . . ?
 O9 Ni1 K1 122.97(19) . . ?
 O9 Ni1 O1 78.2(3) . . ?
 O12 Ni1 Nb1 85.16(19) 2_755 . ?
 O12 Ni1 Nb1 39.01(19) 2_755 2_755 ?
 O12 Ni1 Nb2 39.81(18) 2_755 . ?
 O12 Ni1 K1 122.81(19) 2_755 . ?
 O12 Ni1 O1 78.2(3) 2_755 . ?
 O12 Ni1 O9 77.1(3) 2_755 . ?
 O30 Ni1 Nb1 131.8(3) . . ?
 O30 Ni1 Nb1 131.9(3) . 2_755 ?
 O30 Ni1 Nb2 84.1(3) . . ?
 O30 Ni1 K1 131.1(3) . . ?
 O30 Ni1 O1 169.7(3) . . ?
 O30 Ni1 O9 93.8(3) . . ?
 O30 Ni1 O12 93.9(3) . 2_755 ?
 Nb4 Ni2 Nb6 67.51(3) . . ?
 Nb7 Ni2 Nb4 84.30(4) . . ?
 Nb7 Ni2 Nb6 120.68(4) . . ?
 Nb8 Ni2 Nb4 120.39(4) . . ?
 Nb8 Ni2 Nb6 83.27(4) . . ?
 Nb8 Ni2 Nb7 67.38(3) . . ?
 O2 Ni2 Nb4 88.49(17) . . ?
 O2 Ni2 Nb6 42.39(17) . . ?
 O2 Ni2 Nb7 88.54(17) . . ?
 O2 Ni2 Nb8 42.27(17) . . ?
 O3 Ni2 Nb4 42.50(16) . . ?
 O3 Ni2 Nb6 89.42(16) . . ?
 O3 Ni2 Nb7 42.81(15) . . ?
 O3 Ni2 Nb8 89.37(16) . . ?
 O3 Ni2 O2 80.7(2) . . ?
 O4 Ni2 Nb4 87.21(19) . . ?
 O4 Ni2 Nb6 138.5(2) . . ?
 O4 Ni2 Nb7 86.8(2) . . ?
 O4 Ni2 Nb8 138.1(2) . . ?
 O4 Ni2 O2 174.0(3) . . ?
 O4 Ni2 O3 93.2(2) . . ?
 O4 Ni2 O7 99.0(3) . . ?
 O4 Ni2 O10 98.1(3) . . ?
 O4 Ni2 O31 91.9(3) . . ?
 O7 Ni2 Nb4 40.69(18) . . ?
 O7 Ni2 Nb6 40.77(18) . . ?
 O7 Ni2 Nb7 123.60(18) . . ?
 O7 Ni2 Nb8 122.70(18) . . ?
 O7 Ni2 O2 80.4(2) . . ?
 O7 Ni2 O3 80.8(2) . . ?
 O7 Ni2 O10 155.5(3) . . ?
 O7 Ni2 O31 97.5(3) . . ?
 O10 Ni2 Nb4 123.37(18) . . ?
 O10 Ni2 Nb6 123.08(18) . . ?
 O10 Ni2 Nb7 40.40(17) . . ?
 O10 Ni2 Nb8 41.10(18) . . ?
 O10 Ni2 O2 80.7(2) . . ?
 O10 Ni2 O3 80.9(2) . . ?
 O10 Ni2 O31 99.4(3) . . ?
 O31 Ni2 Nb4 137.0(3) . . ?
 O31 Ni2 Nb6 86.1(3) . . ?
 O31 Ni2 Nb7 138.7(3) . . ?
 O31 Ni2 Nb8 87.5(3) . . ?
 O31 Ni2 O2 94.1(3) . . ?
 O31 Ni2 O3 174.8(3) . . ?
 Nb4 Ni3 Nb4 63.94(4) . 6_565 ?
 Nb4 Ni3 Nb7 115.28(5) . 6_565 ?
 Nb4 Ni3 Nb7 82.20(3) . . ?
 Nb4 Ni3 Nb7 82.20(3) 6_565 6_565 ?
 Nb4 Ni3 Nb7 115.28(5) 6_565 . ?
 Nb4 Ni3 Nb8 115.97(2) 6_565 6_565 ?
 Nb4 Ni3 Nb8 115.97(2) . . ?
 Nb4 Ni3 Nb8 179.05(6) 6_565 . ?
 Nb4 Ni3 Nb8 179.05(6) . 6_565 ?
 Nb7 Ni3 Nb7 64.20(4) . 6_565 ?
 Nb7 Ni3 Nb8 98.64(5) 6_565 . ?
 Nb7 Ni3 Nb8 65.56(3) 6_565 6_565 ?
 Nb7 Ni3 Nb8 65.56(3) . . ?
 Nb7 Ni3 Nb8 98.64(5) . 6_565 ?
 Nb8 Ni3 Nb8 64.09(4) 6_565 . ?
 O2 Ni3 Nb4 138.74(19) . 6_565 ?
 O2 Ni3 Nb4 87.60(18) . . ?
 O2 Ni3 Nb4 87.60(18) 6_565 6_565 ?
 O2 Ni3 Nb4 138.74(19) 6_565 . ?
 O2 Ni3 Nb7 87.45(18) 6_565 6_565 ?
 O2 Ni3 Nb7 138.77(19) . 6_565 ?
 O2 Ni3 Nb7 87.45(18) . . ?
 O2 Ni3 Nb7 138.77(19) 6_565 . ?
 O2 Ni3 Nb8 40.47(17) 6_565 6_565 ?
 O2 Ni3 Nb8 40.47(17) . . ?
 O2 Ni3 Nb8 91.98(18) 6_565 . ?
 O2 Ni3 Nb8 91.99(18) . 6_565 ?
 O2 Ni3 O2 97.1(4) . 6_565 ?
 O2 Ni3 O3 179.6(3) 6_565 . ?
 O2 Ni3 O3 82.6(2) . . ?
 O2 Ni3 O3 179.6(3) . 6_565 ?
 O2 Ni3 O3 82.6(2) 6_565 6_565 ?
 O3 Ni3 Nb4 41.19(16) 6_565 6_565 ?
 O3 Ni3 Nb4 92.60(17) 6_565 . ?
 O3 Ni3 Nb4 92.60(17) . 6_565 ?
 O3 Ni3 Nb4 41.19(16) . . ?
 O3 Ni3 Nb7 92.88(17) . 6_565 ?
 O3 Ni3 Nb7 41.35(16) . . ?
 O3 Ni3 Nb7 41.36(16) 6_565 6_565 ?
 O3 Ni3 Nb7 92.88(17) 6_565 . ?
 O3 Ni3 Nb8 139.59(17) 6_565 . ?
 O3 Ni3 Nb8 87.81(16) . . ?
 O3 Ni3 Nb8 87.81(16) 6_565 6_565 ?
 O3 Ni3 Nb8 139.59(17) . 6_565 ?
 O3 Ni3 O3 97.8(3) 6_565 . ?
 O8 Ni3 Nb4 48.93(17) . 6_565 ?
 O8 Ni3 Nb4 48.93(18) . . ?
 O8 Ni3 Nb7 131.13(18) . 6_565 ?
 O8 Ni3 Nb7 131.13(18) . . ?
 O8 Ni3 Nb8 130.23(18) . 6_565 ?
 O8 Ni3 Nb8 130.23(18) . . ?
 O8 Ni3 O2 90.0(2) . . ?
 O8 Ni3 O2 90.0(2) . 6_565 ?
 O8 Ni3 O3 89.9(2) . 6_565 ?
 O8 Ni3 O3 89.9(2) . . ?
 O8 Ni3 O11 179.8(4) . . ?
 O11 Ni3 Nb4 130.94(18) . . ?
 O11 Ni3 Nb4 130.94(19) . 6_565 ?
 O11 Ni3 Nb7 48.74(18) . . ?
 O11 Ni3 Nb7 48.74(18) . 6_565 ?
 O11 Ni3 Nb8 49.91(18) . . ?
 O11 Ni3 Nb8 49.91(18) . 6_565 ?
 O11 Ni3 O2 90.2(2) . . ?
 O11 Ni3 O2 90.2(2) . 6_565 ?
 O11 Ni3 O3 89.9(2) . 6_565 ?
 O11 Ni3 O3 89.9(2) . . ?
 O1 K1 K1 180.0 . 5_765 ?
 O1 K1 O3 91.76(12) . . ?
 O1 K1 O3 91.76(12) . 2_755 ?
 O1 K1 O13 123.43(10) . . ?
 O1 K1 O13 123.43(10) . 5_765 ?
 O1 K1 O14 122.95(11) . 5_765 ?
 O1 K1 O14 122.95(11) . . ?
 O3 K1 K1 88.24(12) 2_755 5_765 ?
 O3 K1 K1 88.24(12) . 5_765 ?
 O3 K1 O3 176.5(2) . 2_755 ?
 O3 K1 O14 123.0(2) . 5_765 ?
 O3 K1 O14 123.0(2) 2_755 . ?
 O3 K1 O14 54.67(19) 2_755 5_765 ?
 O3 K1 O14 54.67(19) . . ?
 O5 K1 K1 114.79(14) . 5_765 ?
 O5 K1 K1 114.79(14) 2_755 5_765 ?
 O5 K1 O1 65.21(14) . . ?
 O5 K1 O1 65.21(14) 2_755 . ?
 O5 K1 O3 59.44(17) . . ?
 O5 K1 O3 122.28(17) . 2_755 ?
 O5 K1 O3 59.44(17) 2_755 2_755 ?
 O5 K1 O3 122.28(17) 2_755 . ?
 O5 K1 O5 130.4(3) . 2_755 ?
 O5 K1 O13 93.7(2) . 5_765 ?
 O5 K1 O13 113.4(2) 2_755 5_765 ?
 O5 K1 O13 93.7(2) 2_755 . ?
 O5 K1 O13 113.4(2) . . ?
 O5 K1 O14 58.12(16) 2_755 5_765 ?
 O5 K1 O14 169.8(2) . 5_765 ?
 O5 K1 O14 58.12(16) . . ?
 O5 K1 O14 169.8(2) 2_755 . ?
 O6 K1 K1 115.05(14) 2_755 5_765 ?
 O6 K1 K1 115.05(14) . 5_765 ?
 O6 K1 O1 64.95(14) 2_755 . ?
 O6 K1 O1 64.95(14) . . ?
 O6 K1 O3 60.16(17) . . ?
 O6 K1 O3 60.17(17) 2_755 2_755 ?
 O6 K1 O3 121.57(17) . 2_755 ?
 O6 K1 O3 121.57(17) 2_755 . ?
 O6 K1 O5 62.15(19) 2_755 . ?
 O6 K1 O5 96.44(19) 2_755 2_755 ?
 O6 K1 O5 96.4(2) . . ?
 O6 K1 O5 62.15(19) . 2_755 ?
 O6 K1 O6 129.9(3) 2_755 . ?
 O6 K1 O13 58.97(16) . . ?
 O6 K1 O13 169.1(2) . 5_765 ?
 O6 K1 O13 169.1(2) 2_755 . ?
 O6 K1 O13 58.97(16) 2_755 5_765 ?
 O6 K1 O14 92.9(2) . 5_765 ?
 O6 K1 O14 114.2(2) . . ?
 O6 K1 O14 92.9(2) 2_755 . ?
 O6 K1 O14 114.2(2) 2_755 5_765 ?
 O13 K1 K1 56.57(10) 5_765 5_765 ?
 O13 K1 K1 56.57(10) . 5_765 ?
 O13 K1 O3 123.0(2) 5_765 . ?
 O13 K1 O3 123.0(2) . 2_755 ?
 O13 K1 O3 54.67(19) . . ?
 O13 K1 O3 54.67(19) 5_765 2_755 ?
 O13 K1 O13 113.1(2) 5_765 . ?
 O13 K1 O14 76.7(2) . . ?
 O13 K1 O14 76.7(2) 5_765 5_765 ?
 O13 K1 O14 68.4(2) . 5_765 ?
 O13 K1 O14 68.4(2) 5_765 . ?
 O14 K1 K1 57.05(11) 5_765 5_765 ?
 O14 K1 K1 57.05(11) . 5_765 ?
 O14 K1 O14 114.1(2) . 5_765 ?
 Nb3 K2 Nb9 107.31(8) 7_755 . ?
 K3 K2 Nb3 58.66(8) . 7_755 ?
 K3 K2 Nb9 57.40(11) . . ?
 Na1 K2 Nb3 87.74(10) 7_755 7_755 ?
 Na1 K2 Nb9 88.03(10) 7_755 . ?
 Na1 K2 K3 113.13(14) 7_755 . ?
 O28 K2 Nb3 104.5(2) . 7_755 ?
 O28 K2 Nb9 19.87(16) . . ?
 O28 K2 K3 47.1(2) . . ?
 O28 K2 Na1 107.7(2) . 7_755 ?
 O28 K2 O4W 81.4(3) . 7_755 ?
 O28 K2 O6W 86.9(3) . . ?
 O28 K2 O8W 147.8(3) . 7_755 ?
 O28 K2 O13W 77.4(4) . 1_655 ?
 O28 K2 O14W 112.1(5) . 1_655 ?
 O28 K2 O18W 129.9(5) . 1_655 ?
 O33 K2 Nb3 20.06(15) 7_755 7_755 ?
 O33 K2 Nb9 102.8(2) 7_755 . ?
 O33 K2 K3 46.82(19) 7_755 . ?
 O33 K2 Na1 107.3(2) 7_755 7_755 ?
 O33 K2 O28 93.8(3) 7_755 . ?
 O33 K2 O4W 79.6(3) 7_755 7_755 ?
 O33 K2 O6W 145.2(3) 7_755 . ?
 O33 K2 O8W 88.4(3) 7_755 7_755 ?
 O33 K2 O13W 98.4(5) 7_755 1_655 ?
 O33 K2 O14W 150.6(4) 7_755 1_655 ?
 O33 K2 O18W 65.7(5) 7_755 1_655 ?
 O4W K2 Nb3 65.37(18) 7_755 7_755 ?
 O4W K2 Nb9 66.32(19) 7_755 . ?
 O4W K2 K3 73.0(2) 7_755 . ?
 O4W K2 Na1 40.1(2) 7_755 7_755 ?
 O4W K2 O6W 66.1(3) 7_755 . ?
 O4W K2 O14W 116.6(3) 7_755 1_655 ?
 O6W K2 Nb3 127.4(2) . 7_755 ?
 O6W K2 Nb9 69.29(18) . . ?
 O6W K2 K3 122.1(2) . . ?
 O6W K2 Na1 40.8(2) . 7_755 ?
 O6W K2 O14W 54.1(4) . 1_655 ?
 O8W K2 Nb3 70.26(19) 7_755 7_755 ?
 O8W K2 Nb9 129.2(3) 7_755 . ?
 O8W K2 K3 124.7(2) 7_755 . ?
 O8W K2 Na1 41.9(2) 7_755 7_755 ?
 O8W K2 O4W 67.5(3) 7_755 7_755 ?
 O8W K2 O6W 73.7(3) 7_755 . ?
 O8W K2 O13W 134.1(4) 7_755 1_655 ?
 O8W K2 O14W 77.0(4) 7_755 1_655 ?
 O8W K2 O18W 79.9(5) 7_755 1_655 ?
 O13W K2 Nb3 117.0(5) 1_655 7_755 ?
 O13W K2 Nb9 93.6(4) 1_655 . ?
 O13W K2 K3 89.9(3) 1_655 . ?
 O13W K2 Na1 153.2(4) 1_655 7_755 ?
 O13W K2 O4W 158.5(4) 1_655 7_755 ?
 O13W K2 O6W 115.6(5) 1_655 . ?
 O13W K2 O14W 75.2(5) 1_655 1_655 ?
 O13W K2 O18W 62.5(6) 1_655 1_655 ?
 O14W K2 Nb3 143.2(4) 1_655 7_755 ?
 O14W K2 Nb9 106.2(4) 1_655 . ?
 O14W K2 K3 157.6(4) 1_655 . ?
 O14W K2 Na1 78.6(3) 1_655 7_755 ?
 O18W K2 Nb3 72.0(4) 1_655 7_755 ?
 O18W K2 Nb9 149.8(4) 1_655 . ?
 O18W K2 K3 101.6(4) 1_655 . ?
 O18W K2 Na1 121.7(5) 1_655 7_755 ?
 O18W K2 O4W 132.7(5) 1_655 7_755 ?
 O18W K2 O6W 136.2(5) 1_655 . ?
 O18W K2 O14W 86.5(6) 1_655 1_655 ?
 Nb3 K3 Nb3 117.86(17) 4_755 7_755 ?
 Nb9 K3 Nb3 118.23(8) . 7_755 ?
 Nb9 K3 Nb3 118.23(8) . 4_755 ?
 Nb9 K3 K2 65.18(10) . . ?
 Nb9 K3 K2 65.18(10) . 6_565 ?
 K2 K3 Nb3 122.77(17) . 4_755 ?
 K2 K3 Nb3 122.77(17) 6_565 7_755 ?
 K2 K3 Nb3 64.17(7) 6_565 4_755 ?
 K2 K3 Nb3 64.17(7) . 7_755 ?
 K2 K3 K2 69.54(14) . 6_565 ?
 Na2 K3 Nb3 96.97(12) . 4_755 ?
 Na2 K3 Nb3 96.97(12) . 7_755 ?
 Na2 K3 Nb9 100.0(2) . . ?
 Na2 K3 K2 140.19(13) . . ?
 Na2 K3 K2 140.19(13) . 6_565 ?
 O28 K3 Nb3 109.80(13) . 4_755 ?
 O28 K3 Nb3 109.80(13) . 7_755 ?
 O28 K3 Nb9 25.4(2) . . ?
 O28 K3 K2 47.00(15) . . ?
 O28 K3 K2 47.00(15) . 6_565 ?
 O28 K3 Na2 125.4(3) . . ?
 O28 K3 O2W 165.9(4) . 3 ?
 O28 K3 O3W 99.9(3) . 6_565 ?
 O28 K3 O3W 99.9(3) . . ?
 O33 K3 Nb3 110.1(2) 7_755 4_755 ?
 O33 K3 Nb3 24.31(16) 4_755 4_755 ?
 O33 K3 Nb3 24.31(16) 7_755 7_755 ?
 O33 K3 Nb3 110.1(2) 4_755 7_755 ?
 O33 K3 Nb9 110.1(2) 4_755 . ?
 O33 K3 Nb9 110.1(2) 7_755 . ?
 O33 K3 K2 46.46(18) 7_755 . ?
 O33 K3 K2 98.5(2) 4_755 . ?
 O33 K3 K2 98.5(2) 7_755 6_565 ?
 O33 K3 K2 46.46(18) 4_755 6_565 ?
 O33 K3 Na2 121.3(2) 7_755 . ?
 O33 K3 Na2 121.3(2) 4_755 . ?
 O33 K3 O28 93.3(3) 7_755 . ?
 O33 K3 O28 93.3(3) 4_755 . ?
 O33 K3 O33 94.3(4) 4_755 7_755 ?
 O33 K3 O2W 96.2(3) 4_755 3 ?
 O33 K3 O2W 96.2(3) 7_755 3 ?
 O33 K3 O3W 162.6(3) 7_755 6_565 ?
 O33 K3 O3W 96.2(3) 7_755 . ?
 O33 K3 O3W 162.6(3) 4_755 . ?
 O33 K3 O3W 96.2(3) 4_755 6_565 ?
 O2W K3 Nb3 76.48(16) 3 4_755 ?
 O2W K3 Nb3 76.48(16) 3 7_755 ?
 O2W K3 Nb9 140.5(3) 3 . ?
 O2W K3 K2 140.62(16) 3 . ?
 O2W K3 K2 140.62(16) 3 6_565 ?
 O2W K3 Na2 40.5(3) 3 . ?
 O3W K3 Nb3 138.3(3) 6_565 7_755 ?
 O3W K3 Nb3 76.05(19) . 7_755 ?
 O3W K3 Nb3 138.3(3) . 4_755 ?
 O3W K3 Nb3 76.05(19) 6_565 4_755 ?
 O3W K3 Nb9 79.2(2) 6_565 . ?
 O3W K3 Nb9 79.2(2) . . ?
 O3W K3 K2 98.9(2) 6_565 6_565 ?
 O3W K3 K2 144.3(3) . 6_565 ?
 O3W K3 K2 98.9(2) . . ?
 O3W K3 K2 144.3(3) 6_565 . ?
 O3W K3 Na2 41.3(2) . . ?
 O3W K3 Na2 41.3(2) 6_565 . ?
 O3W K3 O2W 68.8(3) . 3 ?
 O3W K3 O2W 68.8(3) 6_565 3 ?
 O3W K3 O3W 70.4(4) . 6_565 ?
 K2 K4 K2 63.20(13) 7_755 4_745 ?
 K3 K4 K2 56.45(12) 7_755 7_755 ?
 K3 K4 K2 56.45(12) 7_755 4_745 ?
 Na2 K4 K2 141.75(14) 3_444 4_745 ?
 Na2 K4 K2 141.75(14) 3_444 7_755 ?
 Na2 K4 K3 107.7(2) 3_444 7_755 ?
 O33 K4 K2 41.65(17) 6 4_745 ?
 O33 K4 K2 90.0(2) 6 7_755 ?
 O33 K4 K2 90.0(2) . 4_745 ?
 O33 K4 K2 41.65(17) . 7_755 ?
 O33 K4 K3 45.53(19) . 7_755 ?
 O33 K4 K3 45.53(19) 6 7_755 ?
 O33 K4 Na2 101.1(2) . 3_444 ?
 O33 K4 Na2 101.1(2) 6 3_444 ?
 O33 K4 O33 91.0(4) 6 . ?
 O33 K4 O2W 73.8(3) 6 . ?
 O33 K4 O2W 73.8(3) . . ?
 O33 K4 O5W 84.5(3) . . ?
 O33 K4 O5W 138.5(4) . 6 ?
 O33 K4 O5W 138.5(4) 6 . ?
 O33 K4 O5W 84.5(3) 6 6 ?
 O33 K4 O18W 133.0(5) 6 7_655 ?
 O33 K4 O18W 64.2(4) 6 4_645 ?
 O33 K4 O18W 133.0(5) . 4_645 ?
 O33 K4 O18W 64.2(4) . 7_655 ?
 O2W K4 K2 113.4(3) . 4_745 ?
 O2W K4 K2 113.4(3) . 7_755 ?
 O2W K4 K3 68.2(3) . 7_755 ?
 O2W K4 Na2 39.4(3) . 3_444 ?
 O5W K4 K2 174.5(2) 6 7_755 ?
 O5W K4 K2 111.9(2) . 7_755 ?
 O5W K4 K2 174.5(2) . 4_745 ?
 O5W K4 K2 111.9(2) 6 4_745 ?
 O5W K4 K3 119.0(3) . 7_755 ?
 O5W K4 K3 119.0(3) 6 7_755 ?
 O5W K4 Na2 40.6(2) . 3_444 ?
 O5W K4 Na2 40.6(2) 6 3_444 ?
 O5W K4 O2W 65.4(3) . . ?
 O5W K4 O2W 65.4(3) 6 . ?
 O5W K4 O5W 72.8(4) . 6 ?
 O5W K4 O18W 81.1(5) . 7_655 ?
 O5W K4 O18W 140.7(5) . 4_645 ?
 O5W K4 O18W 81.1(5) 6 4_645 ?
 O5W K4 O18W 140.7(5) 6 7_655 ?
 O18W K4 K2 96.2(4) 4_645 7_755 ?
 O18W K4 K2 44.5(4) 4_645 4_745 ?
 O18W K4 K2 44.5(4) 7_655 7_755 ?
 O18W K4 K2 96.2(4) 7_655 4_745 ?
 O18W K4 K3 99.1(4) 4_645 7_755 ?
 O18W K4 K3 99.1(4) 7_655 7_755 ?
 O18W K4 Na2 121.7(4) 7_655 3_444 ?
 O18W K4 Na2 121.7(4) 4_645 3_444 ?
 O18W K4 O2W 128.1(4) 7_655 . ?
 O18W K4 O2W 128.1(4) 4_645 . ?
 O18W K4 O18W 103.2(9) 7_655 4_645 ?
 Nb4 K5 Nb4 49.48(7) 2_755 5_765 ?
 Nb4 K5 K1 69.26(9) 5_765 . ?
 Nb4 K5 K1 48.07(6) 2_755 . ?
 Nb7 K5 Nb4 114.68(13) . 5_765 ?
 Nb7 K5 Nb4 92.24(9) 6_565 5_765 ?
 Nb7 K5 Nb4 92.24(9) . 2_755 ?
 Nb7 K5 Nb4 114.68(13) 6_565 2_755 ?
 Nb7 K5 Nb7 53.75(8) . 6_565 ?
 Nb7 K5 K1 71.39(9) 6_565 . ?
 Nb7 K5 K1 48.82(6) . . ?
 O13 K5 Nb4 89.3(2) . 2_755 ?
 O13 K5 Nb4 89.3(2) . 5_765 ?
 O13 K5 Nb7 31.54(11) . 6_565 ?
 O13 K5 Nb7 31.54(11) . . ?
 O13 K5 K1 41.91(17) . . ?
 O13 K5 O14 74.9(3) . 5_765 ?
 O13 K5 O20 56.7(2) . . ?
 O13 K5 O20 56.7(2) . 6_565 ?
 O13 K5 O11W 139.2(2) . 2_755 ?
 O13 K5 O11W 139.2(2) . 5_765 ?
 O13 K5 O15W 120.0(5) . . ?
 O14 K5 Nb4 28.37(10) 5_765 2_755 ?
 O14 K5 Nb4 28.37(10) 5_765 5_765 ?
 O14 K5 Nb7 91.8(2) 5_765 6_565 ?
 O14 K5 Nb7 91.8(2) 5_765 . ?
 O14 K5 K1 43.31(17) 5_765 . ?
 O14 K5 O20 123.3(2) 5_765 . ?
 O14 K5 O20 123.3(2) 5_765 6_565 ?
 O14 K5 O11W 96.8(3) 5_765 5_765 ?
 O14 K5 O11W 96.8(3) 5_765 2_755 ?
 O20 K5 Nb4 145.5(2) 6_565 2_755 ?
 O20 K5 Nb4 117.72(14) 6_565 5_765 ?
 O20 K5 Nb4 145.5(2) . 5_765 ?
 O20 K5 Nb4 117.72(14) . 2_755 ?
 O20 K5 Nb7 31.73(12) 6_565 6_565 ?
 O20 K5 Nb7 31.73(12) . . ?
 O20 K5 Nb7 62.44(15) 6_565 . ?
 O20 K5 Nb7 62.44(15) . 6_565 ?
 O20 K5 K1 80.04(15) . . ?
 O20 K5 K1 98.57(17) 6_565 . ?
 O20 K5 O20 50.8(2) 6_565 . ?
 O11W K5 Nb4 70.4(2) 5_765 2_755 ?
 O11W K5 Nb4 101.9(3) 2_755 2_755 ?
 O11W K5 Nb4 101.9(3) 5_765 5_765 ?
 O11W K5 Nb4 70.4(2) 2_755 5_765 ?
 O11W K5 Nb7 163.7(3) 2_755 . ?
 O11W K5 Nb7 163.7(3) 5_765 6_565 ?
 O11W K5 Nb7 111.9(2) 5_765 . ?
 O11W K5 Nb7 111.9(2) 2_755 6_565 ?
 O11W K5 K1 106.0(2) 5_765 . ?
 O11W K5 K1 139.6(3) 2_755 . ?
 O11W K5 O20 138.8(3) 2_755 . ?
 O11W K5 O20 101.3(3) 2_755 6_565 ?
 O11W K5 O20 138.8(3) 5_765 6_565 ?
 O11W K5 O20 101.3(3) 5_765 . ?
 O11W K5 O11W 80.8(5) 2_755 5_765 ?
 O15W K5 Nb4 142.4(3) . 5_765 ?
 O15W K5 Nb4 142.4(3) . 2_755 ?
 O15W K5 Nb7 101.4(4) . 6_565 ?
 O15W K5 Nb7 101.4(4) . . ?
 O15W K5 K1 148.3(3) . . ?
 O15W K5 O14 165.1(5) . 5_765 ?
 O15W K5 O20 69.7(4) . . ?
 O15W K5 O20 69.7(4) . 6_565 ?
 O15W K5 O11W 72.1(4) . 5_765 ?
 O15W K5 O11W 72.1(4) . 2_755 ?
 Na2 K6 Nb8 83.65(17) . . ?
 O24 K6 Nb8 102.7(2) 7_755 . ?
 O24 K6 Na2 103.1(3) 7_755 . ?
 O24 K6 O3W 76.3(3) 7_755 . ?
 O24 K6 O5W 84.2(3) 7_755 8 ?
 O24 K6 O9W 141.7(4) 7_755 . ?
 O24 K6 O20W 116.7(6) 7_755 . ?
 O24 K6 O22W 152.4(10) 7_755 . ?
 O27 K6 Nb8 17.88(16) . . ?
 O27 K6 Na2 100.6(3) . . ?
 O27 K6 O24 93.3(3) . 7_755 ?
 O27 K6 O3W 72.5(3) . . ?
 O27 K6 O5W 138.3(3) . 8 ?
 O27 K6 O9W 84.2(4) . . ?
 O27 K6 O20W 58.2(5) . . ?
 O27 K6 O22W 89.9(10) . . ?
 O3W K6 Nb8 61.12(19) . . ?
 O3W K6 Na2 40.5(2) . . ?
 O3W K6 O20W 128.8(6) . . ?
 O5W K6 Nb8 123.3(3) 8 . ?
 O5W K6 Na2 40.9(2) 8 . ?
 O5W K6 O3W 66.5(3) 8 . ?
 O5W K6 O20W 155.2(6) 8 . ?
 O9W K6 Nb8 67.4(3) . . ?
 O9W K6 Na2 40.9(4) . . ?
 O9W K6 O3W 66.4(4) . . ?
 O9W K6 O5W 73.2(4) . 8 ?
 O9W K6 O20W 94.3(6) . . ?
 O9W K6 O22W 65.9(10) . . ?
 O20W K6 Nb8 67.7(5) . . ?
 O20W K6 Na2 134.6(6) . . ?
 O22W K6 Nb8 88.4(9) . . ?
 O22W K6 Na2 103.3(9) . . ?
 O22W K6 O3W 130.4(9) . . ?
 O22W K6 O5W 111.0(10) . 8 ?
 O22W K6 O20W 44.4(10) . . ?
 Na1 Na1 K2 143.5(2) 7_755 7_755 ?
 O1W Na1 K2 125.0(2) 7_755 7_755 ?
 O1W Na1 K2 123.9(2) . 7_755 ?
 O1W Na1 Na1 45.2(2) 7_755 7_755 ?
 O1W Na1 Na1 45.2(2) . 7_755 ?
 O1W Na1 O1W 90.5(3) . 7_755 ?
 O1W Na1 O8W 172.2(4) 7_755 . ?
 O1W Na1 O8W 91.3(3) . . ?
 O4W Na1 K2 51.5(3) . 7_755 ?
 O4W Na1 Na1 92.0(3) . 7_755 ?
 O4W Na1 O1W 91.2(3) . . ?
 O4W Na1 O1W 91.7(3) . 7_755 ?
 O4W Na1 O6W 82.8(4) . 7_755 ?
 O4W Na1 O8W 80.7(3) . . ?
 O6W Na1 K2 52.4(3) 7_755 7_755 ?
 O6W Na1 Na1 133.7(3) 7_755 7_755 ?
 O6W Na1 O1W 173.9(4) 7_755 . ?
 O6W Na1 O1W 88.8(3) 7_755 7_755 ?
 O6W Na1 O8W 88.6(4) 7_755 . ?
 O7W Na1 K2 122.7(3) 7_755 7_755 ?
 O7W Na1 Na1 93.8(3) 7_755 7_755 ?
 O7W Na1 O1W 93.5(3) 7_755 . ?
 O7W Na1 O1W 91.9(3) 7_755 7_755 ?
 O7W Na1 O4W 174.1(4) 7_755 . ?
 O7W Na1 O6W 92.5(4) 7_755 7_755 ?
 O7W Na1 O8W 95.6(4) 7_755 . ?
 O8W Na1 K2 48.3(2) . 7_755 ?
 O8W Na1 Na1 136.0(3) . 7_755 ?
 K3 Na2 K4 110.7(3) . 3 ?
 K3 Na2 K6 108.82(18) . . ?
 K3 Na2 K6 108.82(18) . 6_565 ?
 K6 Na2 K4 109.51(18) . 3 ?
 K6 Na2 K4 109.51(18) 6_565 3 ?
 K6 Na2 K6 109.4(3) . 6_565 ?
 O2W Na2 K3 54.5(4) 3 . ?
 O2W Na2 K4 56.2(4) 3 3 ?
 O2W Na2 K6 125.28(15) 3 6_565 ?
 O2W Na2 K6 125.28(15) 3 . ?
 O2W Na2 O3W 87.4(5) 3 . ?
 O2W Na2 O3W 87.4(5) 3 6_565 ?
 O2W Na2 O5W 86.8(4) 3 3 ?
 O2W Na2 O5W 86.8(4) 3 8 ?
 O2W Na2 O9W 173.8(7) 3 . ?
 O3W Na2 K3 51.9(3) . . ?
 O3W Na2 K3 51.9(3) 6_565 . ?
 O3W Na2 K4 125.3(3) . 3 ?
 O3W Na2 K4 125.3(3) 6_565 3 ?
 O3W Na2 K6 56.9(3) . . ?
 O3W Na2 K6 125.2(4) . 6_565 ?
 O3W Na2 K6 125.2(4) 6_565 . ?
 O3W Na2 K6 56.9(3) 6_565 6_565 ?
 O3W Na2 O3W 86.8(6) . 6_565 ?
 O3W Na2 O5W 89.2(4) 6_565 3 ?
 O3W Na2 O5W 173.1(6) . 3 ?
 O3W Na2 O5W 89.2(4) . 8 ?
 O3W Na2 O5W 173.1(6) 6_565 8 ?
 O3W Na2 O9W 88.1(4) . . ?
 O3W Na2 O9W 88.1(4) 6_565 . ?
 O5W Na2 K3 121.3(3) 3 . ?
 O5W Na2 K3 121.3(3) 8 . ?
 O5W Na2 K4 53.5(3) 8 3 ?
 O5W Na2 K4 53.5(3) 3 3 ?
 O5W Na2 K6 56.3(3) 8 . ?
 O5W Na2 K6 56.3(3) 3 6_565 ?
 O5W Na2 K6 129.9(4) 8 6_565 ?
 O5W Na2 K6 129.9(4) 3 . ?
 O5W Na2 O5W 94.2(6) 3 8 ?
 O9W Na2 K3 119.3(5) . . ?
 O9W Na2 K4 129.9(5) . 3 ?
 O9W Na2 K6 54.84(15) . . ?
 O9W Na2 K6 54.84(15) . 6_565 ?
 O9W Na2 O5W 97.4(5) . 8 ?
 O9W Na2 O5W 97.4(5) . 3 ?
 Nb1 O1 Nb1 112.2(4) . 2_755 ?
 Nb1 O1 Ni1 94.64(11) 2_755 2_755 ?
 Nb1 O1 Ni1 94.84(11) 2_755 . ?
 Nb1 O1 Ni1 94.65(11) . . ?
 Nb1 O1 Ni1 94.84(11) . 2_755 ?
 Nb1 O1 K1 123.9(2) . . ?
 Nb1 O1 K1 123.9(2) 2_755 . ?
 Ni1 O1 Ni1 162.9(5) . 2_755 ?
 Ni1 O1 K1 81.5(2) 2_755 . ?
 Ni1 O1 K1 81.5(2) . . ?
 Nb6 O2 Ni2 94.0(3) . . ?
 Nb6 O2 Ni3 98.8(3) . . ?
 Nb8 O2 Nb6 159.6(3) . . ?
 Nb8 O2 Ni2 93.9(3) . . ?
 Nb8 O2 Ni3 98.6(3) . . ?
 Ni3 O2 Ni2 98.4(3) . . ?
 Nb4 O3 Nb7 162.6(3) . . ?
 Nb4 O3 Ni2 93.8(2) . . ?
 Nb4 O3 Ni3 97.4(2) . . ?
 Nb4 O3 K1 81.97(19) . . ?
 Nb7 O3 Ni2 93.4(2) . . ?
 Nb7 O3 Ni3 97.3(2) . . ?
 Nb7 O3 K1 81.15(19) . . ?
 Ni2 O3 K1 128.8(2) . . ?
 Ni3 O3 Ni2 98.3(3) . . ?
 Ni3 O3 K1 132.9(3) . . ?
 Nb1 O4 Ni2 179.2(4) . . ?
 Nb4 O5 Ni1 178.2(4) . 2_755 ?
 Nb4 O5 K1 94.9(3) . . ?
 Ni1 O5 K1 86.2(2) 2_755 . ?
 Nb7 O6 Ni1 177.2(4) . . ?
 Nb7 O6 K1 95.0(3) . . ?
 Ni1 O6 K1 87.2(2) . . ?
 Nb4 O7 Nb6 114.9(3) . . ?
 Nb4 O7 Ni2 98.2(3) . . ?
 Nb6 O7 Ni2 98.2(3) . . ?
 Nb4 O8 Nb4 89.2(3) . 6_565 ?
 Nb4 O8 Nb5 89.6(3) 6_565 . ?
 Nb4 O8 Nb5 89.6(3) . . ?
 Nb4 O8 Nb6 178.1(4) 6_565 . ?
 Nb4 O8 Nb6 91.40(3) 6_565 6_565 ?
 Nb4 O8 Nb6 91.40(3) . . ?
 Nb4 O8 Nb6 178.1(4) . 6_565 ?
 Nb5 O8 Nb6 88.7(2) . . ?
 Nb5 O8 Nb6 88.7(2) . 6_565 ?
 Nb6 O8 Nb6 87.9(3) 6_565 . ?
 Ni3 O8 Nb4 91.0(3) . . ?
 Ni3 O8 Nb4 91.0(3) . 6_565 ?
 Ni3 O8 Nb5 179.2(5) . . ?
 Ni3 O8 Nb6 90.7(3) . . ?
 Ni3 O8 Nb6 90.7(3) . 6_565 ?
 Nb1 O9 Nb2 113.2(3) . . ?
 Nb1 O9 Ni1 98.9(3) . . ?
 Nb2 O9 Ni1 98.8(3) . . ?
 Nb7 O10 Nb8 114.6(3) . . ?
 Nb7 O10 Ni2 98.4(3) . . ?
 Nb8 O10 Ni2 97.5(3) . . ?
 Nb7 O11 Nb7 90.0(3) . 6_565 ?
 Nb7 O11 Nb8 178.5(4) . 6_565 ?
 Nb7 O11 Nb8 178.5(4) 6_565 . ?
 Nb7 O11 Nb8 91.09(3) . . ?
 Nb7 O11 Nb8 91.09(3) 6_565 6_565 ?
 Nb7 O11 Nb9 89.6(3) 6_565 . ?
 Nb7 O11 Nb9 89.6(3) . . ?
 Nb8 O11 Nb8 87.8(3) . 6_565 ?
 Nb9 O11 Nb8 89.3(2) . 6_565 ?
 Nb9 O11 Nb8 89.3(2) . . ?
 Ni3 O11 Nb7 91.0(3) . 6_565 ?
 Ni3 O11 Nb7 91.0(3) . . ?
 Ni3 O11 Nb8 90.0(3) . . ?
 Ni3 O11 Nb8 90.0(3) . 6_565 ?
 Ni3 O11 Nb9 179.1(5) . . ?
 Nb1 O12 Nb2 113.0(3) . 2_755 ?
 Nb1 O12 Ni1 99.1(3) . 2_755 ?
 Nb2 O12 Ni1 98.7(3) 2_755 2_755 ?
 Nb7 O13 Nb7 115.1(4) . 6_565 ?
 Nb7 O13 K1 83.77(16) . . ?
 Nb7 O13 K1 83.77(16) 6_565 5_765 ?
 Nb7 O13 K1 145.2(4) . 5_765 ?
 Nb7 O13 K1 145.2(4) 6_565 . ?
 Nb7 O13 K5 102.4(3) . . ?
 Nb7 O13 K5 102.4(3) 6_565 . ?
 K1 O13 K1 66.9(2) . 5_765 ?
 K5 O13 K1 101.3(3) . . ?
 K5 O13 K1 101.3(3) . 5_765 ?
 Nb4 O14 Nb4 114.8(5) . 6_565 ?
 Nb4 O14 K1 143.5(4) . 5_765 ?
 Nb4 O14 K1 83.55(17) 6_565 5_765 ?
 Nb4 O14 K1 143.5(4) 6_565 . ?
 Nb4 O14 K1 83.55(17) . . ?
 Nb4 O14 K5 107.0(3) . 5_765 ?
 Nb4 O14 K5 107.0(3) 6_565 5_765 ?
 K1 O14 K1 65.9(2) 5_765 . ?
 K5 O14 K1 96.1(3) 5_765 . ?
 K5 O14 K1 96.1(3) 5_765 5_765 ?
 Nb8 O15 Nb9 116.2(3) . . ?
 Nb1 O16 Nb3 115.6(3) . . ?
 Nb1 O17 Nb1 93.9(3) . 2_755 ?
 Nb1 O17 Nb3 88.53(3) . . ?
 Nb1 O17 Nb3 177.6(3) 2_755 . ?
 Nb1 O17 Nb3 177.6(3) . 2_755 ?
 Nb1 O17 Nb3 88.52(3) 2_755 2_755 ?
 Nb2 O17 Nb1 90.73(14) 2_755 . ?
 Nb2 O17 Nb1 90.73(14) . 2_755 ?
 Nb2 O17 Nb1 90.71(14) . . ?
 Nb2 O17 Nb1 90.71(14) 2_755 2_755 ?
 Nb2 O17 Nb2 177.9(4) 2_755 . ?
 Nb2 O17 Nb3 89.24(15) 2_755 2_755 ?
 Nb2 O17 Nb3 89.24(15) . . ?
 Nb2 O17 Nb3 89.26(15) 2_755 . ?
 Nb2 O17 Nb3 89.26(15) . 2_755 ?
 Nb3 O17 Nb3 89.1(3) 2_755 . ?
 Nb4 O18 Nb5 115.2(3) . . ?
 Nb2 O19 Nb3 115.0(4) 2_755 . ?
 Nb7 O20 Nb9 115.4(3) . . ?
 Nb7 O20 K5 89.4(2) . . ?
 Nb9 O20 K5 109.2(2) . . ?
 Nb8 O21 Nb8 117.5(5) . 6_565 ?
 Nb6 O22 Nb6 117.4(5) . 6_565 ?
 Nb2 O23 Nb3 115.0(3) . . ?
 Nb2 O24 K6 129.7(4) . 7_755 ?
 Nb3 O26 Nb3 115.3(4) . 2_755 ?
 Nb8 O27 K6 133.8(4) . . ?
 Nb9 O28 K2 127.4(2) . . ?
 Nb9 O28 K2 127.4(2) . 6_565 ?
 Nb9 O28 K3 111.5(5) . . ?
 K2 O28 K2 102.1(3) 6_565 . ?
 K2 O28 K3 85.9(3) . . ?
 K2 O28 K3 85.9(3) 6_565 . ?
 Nb6 O29 Nb5 115.8(3) . . ?
 Nb3 O33 K2 127.3(4) . 7_755 ?
 Nb3 O33 K3 115.1(4) . 7_755 ?
 Nb3 O33 K4 131.1(4) . . ?
 K2 O33 K3 86.7(3) 7_755 7_755 ?
 K2 O33 K4 94.9(3) 7_755 . ?
 K3 O33 K4 87.3(2) 7_755 . ?
 Na1 O1W Na1 89.5(3) . 7_755 ?
 K3 O2W K4 169.3(5) 3_444 . ?
 Na2 O2W K3 85.0(5) 3_444 3_444 ?
 Na2 O2W K4 84.3(5) 3_444 . ?
 K3 O3W K6 169.3(4) . . ?
 Na2 O3W K3 86.8(4) . . ?
 Na2 O3W K6 82.6(4) . . ?
 Na1 O4W K2 88.4(3) . 7_755 ?
 K4 O5W K6 167.0(4) . 8_454 ?
 Na2 O5W K4 85.9(4) 3_444 . ?
 Na2 O5W K6 82.8(4) 3_444 8_454 ?
 Na1 O6W K2 86.8(3) 7_755 . ?
 Na1 O8W K2 89.8(3) . 7_755 ?
 K6 O9W K6 166.8(7) . 6_565 ?
 Na2 O9W K6 84.2(4) . 6_565 ?
 Na2 O9W K6 84.2(4) . . ?
 K2 O13W K2 98.4(6) 1_455 6_465 ?
 K2 O18W K4 90.3(6) 1_455 7_655 ?

_shelx_SHELXL_version_number      '2014/7'
_olex2_submission_special_instructions 'No special instructions were received'

